# Essentials of crystallography Essentials

Crystallography

By

EDWARD HENRY KRAUS, Ph.D.

\\

Junior Professor of Mineralogy in the

University of Michigan

THE

UNIVERSITY

OF

WITH 427

FIGURES

GEORGE WAHR, Publisher

Ann Arbor, Mich.

1906

by

EDWARD H.

KRAUS

EIL!8 PUBLISHING COMPANY, PRINTEI

BATTIE CRfctK. MICH.

, ra:ma:aOO~\

PREFACE.

This text is intended for beginners and aims to present the

essential features of geometrical crystallography from a standpoint

icm

ERRATA.

Page 26, last line, for 78 31

'

.

ra:ma:OOa1

Page 35, line 8, for + I I read + I

-j-

Page 37, line 6 from the bottom, for effected read affected.

4O2 462

-

Page 42, last line, for A = -f / read A. = +

- /.

2 4

Page 45, line 3, for planes read plane.

Page 47, line 14, for triangle read triangles.

ngures nave oeen muwn

have been taken from various sources.

roi--xKx-i.v,.ft.i.r --v*~

I am indebted to Mr. W. F. Hunt, Instructor in Mineralogy,

also to Messrs. I. D. Scott and C. W. Cook, Assistants in Mineralogy

in the University of Michigan, for aid in the reading of the proof.

EDWARD H. KRAUS.

Mineralogical Laboratory, University of Michigan,

Ann Arbor, Mich., June, 1906.

196447

EIL!8 PUBLISHING COMPANY, PRINTERS

BATTIE CRttK. MICH.

PREFACE.

This text is intended for beginners and aims to present the

essential features of geometrical crystallography from a standpoint

which combines the ideas of symmetry with those of holohedrism,

hemihedrism, etc. All forms possible in the thirty-two classes of

symmetry are discussed even though representatives of several of the

classes have not as yet been observed among minerals or artificial

salts. In each system, however, the important classes are indicated

so that the book may readily be used for abridged courses.

No attempt has been made to discuss the measurement and

projection of crystals inasmuch as they involve a somewhat comprehensive

knowledge of forms and, hence, cannot be treated adequately

in an introductory course. For a similar reason very little reference

has been made to the various structural theories of crystals. However,

the bibliography of the more important works, which have been

published in English and German during the past thirty years, will

prove useful to those who may desire to pursue the study of crystallography

further than the scope of this text permits.

Free use has been made of the various standard texts on crystallography,

but especial acknowledgments are due von Groth, Linck,

Bruhns, Tschermak, and E. S. Dana. A very large majority of the

figures have been drawn especially for this text, the others, however,

have been taken from various sources.

I am indebted to Mr. W. F. Hunt, Instructor in Mineralogy,

also to Messrs. I. D. Scott and C. W. Cook, Assistants in Mineralogy

in the University of Michigan, for aid in the reading of the proof.

EDWARD H. KRAUS.

Mineralogical Laboratory, University of Michigan,

Ann Arbor, Mich., June, 1906.

196447 [in]

INTRODUCTION.

PAGE

Crystals and Crystalline Structure 1

Amorphous Structure 1

Some Properties of Crystallized and Amorphous Substances 2

Crystallography 2

Constancy of Interfacial Angles 2

Crystal Habit 4

Crystallographic Axes 4

Crystal Systems 5

Parameters and Parametral Ratio 5

Fundamental Forms 6

Combinations 7

Axial Ratio 7

Rationality of Coefficients 9

Symbols 10

Symbols of Naumann and Dana 11

Miller's System 12

Elements of Symmetry 12

Planes of Symmetry 12

Axes of Symmetry 13

Center of Symmetry 14

Angular Position of Faces 14

Classes of Symmetry 14

Holohedrism 15

Hemihedrism 15

Tetartohedrism

, 15

Ogdohedrism 15

Correlated Forms 15

Hemimorphism 16

CUBIC SYSTEM.

Crystallographic Axes 17

Classes of Symmetry 17

Hexoctahedral Class (1) 17

Hextetrahedral Class (2) 26

Dyakisdodecahedral Class (3) 32

Pentagonal Icositetrahedral Class (4) 36

Tetrahedral Pentagonal Dodecahedral Class (5) 38

HEXAGONAL SYSTEM.

Crystallographic Axes 43

Classes of Symmetry 44

[V]

VI

Dihexagonal Bipyramidal Class (6) 44

Dihexagonal Pyramidal Class (7) 53

Hexagonal Hemihedrisms 55

Ditrigonal Bipyramidal Class (8) 56

Ditrigonal Scalenohedral Class (9) 60

Hexagonal Bipyramidal Class (10)

6">

Hexagonal Trapezohedral Class (11) 68

Ditrigonal Pyramidal Class (12) 70

Hexagonal Pyramidal Class (13) 74

Hexagonal Tetartohedrisms 76

Trigonal Bipyramidal Class (14) ... 76

Trigonal Trapezohedral Class (15) 81

Trigonal Rhombohedral Class (16) 85

Trigonal Pyramidal Class (17) 89

TETRAGONAL SYSTEM.

Crystallographic Axes 92

Classes of Symmetry 92

Ditetragonal Bipyramidal Class (18) 93

Ditetragonal Pyramidal Class (19) 99

Tetragonal Hemihedrisms 101

Tetragonal Scalenohedral Class (20) 102

Tetragonal Bipyramidal Class (21) 105

Tetragonal Trapezohedral Class (22) 108

Tetragonal Pyramidal Class (23) 110

Tetragonal Bisphenoidal Class (24) Ill

ORTHORHOMBIC SYSTEM.

Crystallographic Axes 115

Classes of Symmetry 115

Orthorhombic Bipyramidal Class (25) 115

Orthorhombic Pyramidal Class (26) 121

Orthorhombic Bisphenoidal Class (27) 123

MONOCUNIC SYSTEM.

Crystallographic Axes 126

Classes of Symmetry 126

Prismatic Class (28)

. . 126

Domatic Class (29) 132

Sphenoidal Class (30) 135

TRICLINIC SYSTEM.

Crystallographic Axes 138

Classes of Symmetry 138

Pinacoidal Class (31) 138

Asymmetric Class (32) 142

VII

COMPOUND CRYSTALS.

Parallel Grouping 144

Twin Crystals 144

Common Twinning Laws

Cubic System 145

Hexagonal System 146

Tetragonal System 147

Orthorhombic System 147

Monoclinic System 147

Triclinic System 148

Repeated Twinning 148

Mimicry 149

TABULAR CLASSIFICATION OF THE THIRTY-TWO

OF CRYSTALS.

CLASSES

Cubic System 150

Hexagonal System 151

Tetragonal System 153

Orthorhombic System 154

Monoclinic System 155

Triclinic System K6

Index .... . 157

Linck, G., Grundriss der Krystallographie, Jena, 1896.

[IX]

BIBLIOGRAPHY.

In the following

list will be found some of the more recent works

which treat crystallography more or less in detail.

Bauer, M., Lehrbuch der Mineralogie, 2d Ed., Stuttgart, 1904.

Bauerman, H., Text Book of Systematic Mineralogy, London, 1881.

Baumhauer, H., Das Reich der Krystalle, Freiburg in Br. , 1884.

Die neuere Entwickelung der Krystallographie,

Leipzig, 1905.

Brezina, A., Methodik der Krystallbestimmung, Vienna, 1884.

Bruhns, W., Elemente der Krystallographie, Liepzig and Vienna,

1902.

Brush-Penfield, Manual of Determinative Mineralogy, New York,

1898.

Dana, E. S., Text Book of Mineralogy, New Edition, New York, 1898.

Fock, A., Introduction to Chemical Crystallography, translated by

W. J. Pope, Oxford, 1895.

Goldschmidt, V., Krystallographische Winkeltabellen, Berlin, 1897.

Index der Krystallformen der Mineralien, 3 vols.,

Berlin, 1886-1891.

Anwendung der Linearprojection zum Berechnen der

Krystalle, Berlin, 1887.

Groth, P., Physikalische Krystallographie, 4th Ed., Leipzig, 1905.

Einleitung in die Chemische Krystallographie, Leipzig,

1904. English Translation by H. Marshall,

New York, 1906.

Heinrich, F. ,

Lehrbuch der Krystallberechnung, Stuttgart, 1886.

Klein, C., Einleitung in die Krystallberechnung, Stuttgart, 1876.

Klockmann, F., Lehrbuch der Mineralogie, 3d Ed., Stuttgart, 1903.

Lewis, W. J., Crystallography, Cambridge, 1899.

Liebisch, T. ,

Geometrische Krystallographie, Leipzig, 1881.

Physikalische Krystallographie, Leipzig, 1891.

Grundriss der Physikalischen Krystallographie, Leipzig,

1896.

X

BIBLIOGRAPHY.

Miers, H. A., Mineralogy, London and New York, 1902.

Moses and Parsons, Mineralogy, Crystallography and Blowpipe

Analysis, Revised Edition, New York, 1904.

Moses, A. J.,

Characters of Crystals, New York, 1899.

Naumann-Zirkel, Elemente der Mineralogie,

1 4th Ed., Leipzig, 1901.

Neis, A., Allgemeine Krystallbeschriebung auf Grund einer vereinfachten

Methode der Krystallzeichnung, Stuttgart,

1895.

Rose, G., Elemente der Krystallographie, 3d Ed., Revised by A.

Sadebeck, A., Angewandte Krystallographie, Berlin, 1876.

Schonflies, A., Krystallsysteme and Krystallstructur, Leipzig, 1891.

Sohncke, L.,

Entwickelung einer Theorie der Krystallstructur, Leipzig,

1879.

Tschermak, G., Lehrbuch der Mineralogie, 6th Ed., Vienna, 1905.

Viola, C., Grundzuge der Kristallographie, Leipzig, 1904.

Voigt, W., Die Fundamentalen Physikalischen Eigenschaften del

Krystalle, Leipzig, 1898.

Von Kobell, F. ,

Lehrbuch der Mineralogie, 6th Ed., Leipzig, 1899.

Websky, M., Anwendung der Linearprojection zum Berechnen del

Krystalle, Berlin, 1887.

Williams, G. H., Elements of Crystallography, 3d Ed., New York

1890.

Wiilfing, E. A. ,

Tabellarische Uebersicht der Einfachen Formen del

32 Krystallographischen Symmetriegruppen,

Stuttgart, 1895.

Also, S. L. Penfield, Stereographic Projection and its Possibilities

from a Graphic Standpoint. American Journa

of Science, 1901, XI, 1-24 and 115-144.

On the Solution of Problems in Crystallography b)

Means of Graphical Methods, Ibid., 1902, XIV,

249-284.

On Crystal Drawing, Ibid., 1905, XIX, 39-75.

UNIVERSITY

* Li FOR N^

INTRODUCTION.^

Crystals and Crystalline Structure, Nearly all homogeneous

substances possessing a definite chemical composition, when solidifying

from either a solution, state of fusion or vapor, attempt to crystallize,

that is, to assume certain characteristic forms. If the process

of solidification is slow enough and uninterrupted, regular forms,

bounded by plane surfaces, usually result. These regular polyhedral

forms are termed crystals. If, however, the solidification is so rapid

that the substance cannot assume well defined forms, bounded by

plane surfaces, the solid mass, which results, is said to be crystalline.

Crystalline substances consist of aggregations of crystals, which have

been hindered in their development. Their outline and orientation

are, hence, irrregular. Figure I shows a well developed crystal of

\

Fig- 1. Fig. 2.

calcite (CaCO3), while figure 2 1 )

represents a cross-section through a

crystalline aggregate of the same substance. Here,

is

no definite outline

to be recognized on the component parts of the mass.

Amorphous Structure. Those substances, however, which do

not attempt to crystallize, when solidifying, are termed amorphous.

i) After Weinschenk. 

2 INTRODUCTION.

They are without form. Opal (SiO 2 x H . 2O), for example, never

occurs in welj. .defined crystals or in crystalline masses.

':

.Some -"Pro'pBrties of Crystallized and Amorphous Substances.

There; are; 'tnany interesting features to be noted in the study of

crystallized and amorphous substances. The attempt at crystallization

and the assuming of regular polyhedral forms, which is characteristic

of bodies belonging to the first class, are only some of the

expressions of the nature of such substances. The various physical

properties, hardness, elasticity, cohesion, transmission of heat and

light, usually vary in such crystallized substances with the direction

according to fixed laws. This is not the case with amorphous substances.

Hence, we may define a crystal as a solid body, which

is bounded by natural -plane surfaces and whose form is

dependent upon its physical and chemical properties.

Crystallography. This science treats of the various properties

of crystals and crystallized bodies. It may be subdivided as follows:

1. Geometrical Crystallography.

2. Physical Crystallography,

j. Chemical Crystallography.

Geometrical crystallography, as the term implies, describes the

various forms occurring upon crystals. The relationships existing

between the crystal form and the physical and chemical properties

of crystals are the subjects of discussion of the second and third subdivisions

of this science, respectively. Only

the essentials of the

first subdivision geometrical crystallography will be treated in

this

text.

Constancy of Interfacial Angles. As indicated on page i,

crystals may, in general, result from solidification from a solution,

that some ammonium

state of fusion, or vapor. Let us suppose

alum, (NH 4) 2A1 2 (SO 4) 4.24H 2O, has been dissolved in water and the

solution allowed to evaporate slowly. As the alum begins to crystallize,

it will be noticed that the crystals are, for the most part, bounded

by eight plane surfaces.

If these surfaces are all of the same size, that

is, have been equally developed, the crystals will possess

an outline

as represented by figure 3. Such a form is termed an octahedron.

The octahedron is bounded by eight equilateral triangles. The

angles between any two adjoining surfaces or faces, as they are often

INTRODUCTION. 3

called, is the same, namely, 109 28^'. On most of the crystals,

Fig. 3. Fig 4. Fig. 5.

Fig. 6. Fig. 7. Fig. 8.

however, it will be seen that the various faces have been developed

unequally, giving rise to the forms illustrated by figures 4 and

5. Similar cross-sections

through these forms are

shown in figures 6, 7, and

8, and it is readily seen

that, although the size

of the faces and, hence,

the resulting shapes have

been materially changed,

the angle between the

F

mained the same, namely,

109 28^'. Such forms

of the octahedron are

said to be misshapen or

distorted. Dist or t ion

is quite common on all

crystals regardless of their

chemical composition.

It was the Danish

physician and natural

Fig. 11. Fig. 12.

9

INTRODUCTION.

scientist, Nicolas Steno, who in 1669 first showed that the angles

between similar faces on crystals of quartz remain constant regardless

of their development. Figures 9 and 10 represent two crystals

of quartz with similar cross-sections (figures 11 and 12). Further

observations, however, showed that this applies not only to quartz but

to all crystallized substances and, hence, we may state the law as

follows: Measured at the same temperature, similar angles on

crystals of the same substance remain constant regardless of

the size or shape of the crystal.

Crystal Habit. The various shapes of crystals, resulting from

the unequal development of their faces, are oftentimes called their

habits. Figures 3, 4, and 5 show some of the habits assumed by

alum crystals. In figure 3, the eight faces are about equally

developed and this may be termed the octahedral habit. The tabular

habit, figure 4, is due to the predominance of two parallel

faces. Figure 5 shows four parallel faces predominating, and the

resulting form is the

prismatic habit.

Crystallographic Axes. Inasmuch as the crystal form of any

substance is

dependent upon its physical and chemical properties, page

2, it

necessarily follows that an almost

infinite variety of forms is possible. In

Fig. 13.

order, however, to study these forms and

define the position of the faces occurring on

definite lengths are assumed to pass through

the ideal center of each crystal. These lines

are the crystallographic axes. Their

intersection forms the axial cross. Figure

13 shows the octahedron referred to its

three crystal axes. In this case the axes

+6.'

-c

Fig. 14.

are of equal lengths and termed a axes.

The extremities of the axes are differentiated

by the use of the plus and minus signs,

as shown in figure 13.

If the axes are of unequal lengths, the

one extending from front to rear is termed

the a axis, the one from right to left the b y

INTRODUCTION. 5

while the vertical axis is called the c axis. This is illustrated by

figure 14. The axes are always referred to in the following order,

viz: a, b, c.

Crystal Systems. Although a great variety of crystal forms is

possible, it has been shown in many ways that all forms may be

classified into six large groups, called crystal systems.

In the grouping

of crystal forms into systems, we are aided by the crystallographic

axes. The systems may be differentiated by means of the axes as

follows :

1. Cubic System. Three axes, all of equal lengths, intersect

at right angles. The axes are designated by the letters, #, a, a.

2. Hexagonal System. Four axes, three of which are equal

and in a horizontal plane intersecting at angles of 60. These three

axes are often termed the

lateral or secondary axes, and are designated

by a, a, a. Perpendicular to the plane of the lateral axes is

the vertical axis, which may be longer or shorter than the a axes.

This fourth axis is called the ^principal or c axis.

3. Tetragonal System. Three axes, two of which are equal,

horizontal, and perpendicular to each other. The vertical, c, axis is

at right angles to and either longer or shorter than the horizontal or

lateral, a,

axes.

4. Orthorhombic System, Three axes of unequal lengths

intersect at right angles. These axes are designated by a, b, c, as

shown in figure 14.

5. Monoclinic System. Three axes, all unequal, two of

which (#', c) intersect at an oblique angle, the third axis (b) being

perpendicular to these two.

6. Triclinic System, Three axes (a, b, c) are all unequal

and intersect at oblique angles.

Parameters and Parametral Ratio,

In order to determine the

position of a face on a crystal, it must be referred to the crystallographic

axes. Figure I 5 shows an axial cross of the orthorhombic

system. The axes, a, b, c, are, therefore, unequal and perpendicular

to each other. The plane ABC cuts the three axes at the points

A, B, and C, hence, at the distance OA a, OB=b, OC=c, from

the center, O. These distances, OA, OB, and OC, are known as

6 INTRODUCTION.

the parameters and the ratio, OA : OB OC, as the parametral

ratio of the plane ABC. This ratio may, however, be abbreviated

to a : b : c.

:

Fig. 15. Fig. 16.

There are,

cross which possess parameters of the same lengths as those of the

plane ABC, figure 16. The simplified ratios of these planes are:

These eight planes, which are similarly located with respect to the

crystallographic axes, constitute a crystal

form, and may be represented by the general

ratio (a b : : c).

The number of faces in a

crystal form depends, moreover, not only upon

the intercepts or parameters but also upon

the elements of symmetry possessed by the

crystal, see page 12. Those forms, which

enclose space, are called closed forms.

Figure 16 is such a form. Those, however,

which do not enclose space on all sides, as

Fig. 17. shown in figure 17, are termed open forms.

Fundamental Form. In figure 18, the enclosed form possesses

the general ratio, a : b : c. The face ABM, however, has the

parametral ratio, oA :

where oA =

,

oB

=

,

INTRODUCTION.

:

oB oM,

and oM =

3oC 3

8 INTRODUCTION.

Aragonite, CaCO 3 ,

a :

Anglesite, PbSO 4 ,

a :

Topaz, A1 2 (F.OH) 2 SiO 4 ,

a

:

b : c = .6228 : i :

.7204

b

: c = .7852

: I :

1.2894

b : ^ = .5281

: I :

.9442

In the hexagonal and tetragonal systems, since the horizontal

axes are all equal, i. c., a = b, see page 5, the axial ratio is reduced

to a :

c; a now being unity. Thus, the axial ratio of zircon (ZrSiO 4)

which is tetragonal, may be expressed as follows: a : c= i :

.6404;

that of quartz (SiO 2 ), hexagonal, by a = c : I :

1.0999. Obviously,

in the cubic system, page 5, where all three axes are equal, this is

unnecessary.

However, in the monoclinic and triclinic systems, where either

one or more axes intersect obliquely, it is not only necessary to give

the axial ratio but also to indicate the values of the angles

between the crystallographic axes. For example, gypsum (CaSO 4

.

2H 2O) crystallizes in the monoclinic system and has the following

axial ratio:

a' : b

:

c :

.6896

I :

.4133

and the inclination of the a' axis to the c is 98 58'. This angle

is known as

, figure 2 1 .

-b-

fb

-c

Fig. 21,

Fig. 22.

In the triclinic system,

since all axes are inclined to each other,

it is also necessary to know the value of the three angles, which are

located as shown in figure 22, viz: b/\c=a, a A c = /?, a A b

=:

The axial ratio and the angles showing the inclination of the axes are

termed the elements of crystallization.

The triclinic mineral albite (NaAlSi 3O 8) possesses the following

elements of crystallization:

a:5:t= .6330

: I :

5573.

= 94 5'

0= 116 27'

y= 88 7'

y.

INTRODUCTION. 9

If the angles between the crystallographic axes equal 90, they

are not indicated. Therefore, in the tetragonal, hexagonal, and

orthorhombic systems, the axial ratios alone constitute the elements

of crystallization, while in the cubic system, there are no unknown

elements.

Fig. 23.

Rationality of Coefficients. The parametral ratio of any face

may be expressed in general by na : :

pb me, where the coefficients

n, p, m< are according to observation always rational. In figure 23,

the inner pyramid

is assumed to be the fundamental form,

page 7, with the following value of the intercepts: oa=i.256,

ob = i, oc .752. But the coefficients n, p, m, are obviously all

equal to unity. The ratio is, Hence, a : b : c.

The outer pyramid, however, possesses the intercepts, oa =

1.256, oJ3 = 2, oC=2.2\$6. These lengths, divided by

the unit

10 INTRODUCTION.

lengths of each axis, as indicated above, determine the values of n,

p, and m for the outer pyramid, namely:

1.256

i

.752

= 3.

These values of n, p, and ;w, are, therefore, rational. Such

values as

,

,_J, f, or f are also possible, but never 3.1416-!-,

2.6578-)-, 1/3, and so forth.

may

Symbols. The parametral ratio of the plane ABM, figure 18,

be written as follows:

na :pb

: me.

If, however, the coefficients had the values |, f ,

and J, respectively,

But since, in this case, n = i, p = i, m = 3, the ratio becomes:

a :

I :

fa

\a : \b : fa

This, when expressed in terms of b,

Hence, the ratio

\a : b : 2c.

na : b : me

becomes:

expresses the most general ratio or symbol for forms belonging to the

orthorhombic, monoclinic, and triclinic systems. In the hexagonal

and tetragonal systems, since the a and b axes are equal, this general

symbol becomes,

a : na : me.

Figure 24 shows

a form, the ditetrag

o n a 1

bipyramid,

Fig. 24.

with the symbol a :

2a :

\c. In the cubic

system, all three axes

are equal and the

general

symbol

a : na : ma.

INTRODUCTION. 11

The ratio a : 00 a :

a, for example, symbolizes a form in the

cubic system consisting of six faces, which cut one axis and extend

parallel to the other two. Such a form

is the cube, figure 25. The ratio a:2a: CD a

represents a form with twenty-four faces;

each face cuts one axis at a unit 's

length,

the second at twice that length, but

extends parallel to the third axis. Figure

26 shows such a form, the tetrahexahedron.

This system of crystallographic

notation is known as the Weiss system

after the inventor Prof. C. S. Weiss.

These symbols are most readily understood

Naumann, Dana, and Miller have introduced

modifications tending to shorten the

symbols of Weiss. Since these shortened

forms are employed quite extensively, it will

be necessary to explain each briefly.

Symbols of Naumann and Dana. In

the notation of Naumann, O and P, the

Fig. 26.

initial letters of the words, octahedron and pyramid, respectively,

are used as a basis. O is used for forms of the cubic system, P for

all other systems. The coefficient m, referring to the vertical axis,

is

placed before and the other coefficient n, after one of these letters.

For example, na : TJ :

m, becomes mPn, and a : ma :

ooa, CQQm.

Dana 's notation is similar to that of Naumanrr. Dana, however,

substitutes a short dash for the letters O and P, also i or I for oo,

the sign of infinity. Otherwise, the two systems are alike.

The following table shows several Weiss symbols with the corresponding

Naumann and Dana modifications:

Weiss

^

2C

\C

oca

oca

ma

Naumann

2Pf

|Pa

ocOoo

OCO2

mOn

Dana

3

-

i-2

m n

12 INTRODUCTION.

Miller's System. In this system,

notations of Naumann and Dana, th\$ letters referring

as is also the case with the

to the various

crystallographic axes are not indicated. The values given being

understood as referring to the a, b, and c axes respectively, page 5.

The reciprocals of the Weiss parameters are reduced to the lowest

common denominator, the numerators then constitute the Miller

symbols, called indices^. For example, the reciprocals of the Weiss

parameters 2a : b : ^c would be |, y, i- These, reduced to the lowest

common denominator, are f , f, f . Hence, 362

constitute the

corresponding Miller indices. These are read three, six, two.

A number of examples will make this system of notation clear.

Thus, a : dob

:

ccc, becomes 100; 2a : b :

\$c, 5.10.2; a : a :

?>c,

331 a :

;

ooa :

2c, 201, and so forth. The Miller indices corresponding

to the general ratios a : no, : ma and na : b : me are written

hkl. The Miller indices are important because of their almost

universal application in crystallographic investigations. The transformation

of the Naumann or Dana symbols to those of Miller should,

after the foregoing explanations, present no difficulty whatever.

Elements of Symmetry. The laws of. symmetry find expression

upon a crystal in the distribution of similar angles and faces.

The presence, therefore, of planes, axes, or a center of symmetry

for the

these are the elements of symmetry

is of great importance

correct classification of a crystal.

Planes of Symmetry. Any plane, which passes through the

Fig. 27.

center of a crystal and divides it into two symmetrical

parts, the one-half being the mirror-image

of the other, is a plane of symmetry. Figure 27

shows a crystal of gypsum (CaSO 4

.2H 2O) with

its one plane of symmetry. Every plane of symmetry

is parallel to some face, which is either

present or possible upon the crystal. In figure

27 it is parallel to the face b.

planes of

It is sometimes convenient to subdivide the

symmetry into principal and secondary

or common planes, according to whether they

possess two or more equivalent and interchangeable

directions or not. Figure 28 illustrates a crystal

of the tetragonal system with five planes of sym-

metry. The horizontal plane c is the

principal, the vertical planes the secondary

planes of symmetry.

Axes of Symmetry. The line, about

which a crystal may be revolved as an axis

so that after a definite angular revolution

the

crystal assumes exactly the same position

in space which it originally had, is

termed an axis of symmetry.

INTRODUCTION. 13

Depending

upon the rotation necessary, only four types

of axes of symmetry are from the stand-

Fig. 28.

point of crystallography possible. 1 '

a) Those axes, about which the original position is reassumed

after a revolution of 60, are said to be axes of hexagonal, six-fold,

or six-count 2 '*

symmetry. Such axes may be indicated by the symbol

.

Figure 29 shows such an axis.

b) If the original position is regained after the crystal is revolved

through 90, the axis is termed a tetragonal, four-count, or fourfold

axis of symmetry. These axes are represented by ,

as illus-

Fig. 29. Fig. 30. Fig. 31.

c) Axes requiring an angular revolution of 120 are trigonal,

three-fold, or three-count axes of symmetry and may be symbolized

by A. Figure 31 illustrates this type of axis.

1) For proof, see Groth's Physikalische Krystallographie, 4te Auflage, 1905, 321; also Viola'*

Grundziige der Kristallographie, 1904, 251.

2) Because in a complete revolution of 360 the position is reassumed six times.

14 INTRODUCTION.

d) A binary, two-fold, or two-count axis necessitates a revolution

through 1 80. These are indicated by in figure 30.

Center of Symmetry. That point within a

crystal through which straight lines may be drawn,

so that on either side of and at the same distance

Fig 3*.

from it, similar portions of the -crystal (faces,

edges, angles, and so forth) are encountered, is a

center of symmetry. Figure 32 has a center of

symmetry the other elements of symmetry are

lacking.

Angular Position of Faces. Since crystals are oftentimes misshapen

or distorted, page 3, it follows that the elements of

symmetry are not

The angular

position of the faces

in respect to these

elements is the

essential feature, and

not their distance or

relative size. Figure

33 shows an ideal

crystal of a u g

i t e.

Here, the presence

Fig. 33. Fig. 34. of a plane of symmetry,

an axis, and a

center of symmetry

is obvious. Figure 34 shows a distorted crystal of

the same mineral, possessing however exactly the same elements of

symmetry, because the angular position of the faces is

figure 33.

the same as in

Classes of Symmetry. Depending upon the elements of symmetry

present, crystals may be divided into thirty-tivo distinct groups,

called classes of symmetry. l)

Only forms which belong to the same

class can occur in combination with each other. A crystal system,

however, includes all those classes of symmetry which can be

referred to the same type of crystallographic axes, page 5. The

l) Also termed classes of crystals.

INTRODUCTION. 15

various elements of symmetry and, wherever possible, an important

representative are given for each of the thirty-two classes in the

tabular classification on page 150.

Holohedrism. Figure 35 shows a form of the cubic system.

The face a b c has the parametral ratio a : \a : 30. Forty-seven

other faces, having this same ratio, are however

also possible and, when present, give rise

to the hexoctahedron, as the complete form

is called. These forty-eight faces are all

equal, scalene triangles. Such forms, which

possess all the faces possible having the same

are called holohedral forms.

ratio,

Hemihedrism. If, however, one-half of

the faces of the hexoctahedron be suppressed

and the other half be allowed to expand, as

shown in figure 36, the diploid with half of

the faces possessed by the hexoctahedron,

namely twenty-four,

character are said to be hemihedral.

results. Forms of this

Tetartohedrism. Again,

if only one

quarter of the faces expand, all others being

suppressed, the hexoctahedron then yields the

tetrahedral pentagonal dodecahedron with

but twelve faces, figure 37. This is a tetartohedral

form.

Ogdohedrism. There are still other

forms, which possess but one-eighth of the

number of faces of the original holohedral

form, and these are termed og-dohedral forms.

Figure 270, page 91, shows such ogdohedral

forms in combination.

Fig. 35.

Fiar 36.

Fig. 37.

It is evident that these complete and partial forms possess different

elements of symmetry and, hence, only those forms which are of

the same type, that is, possess the same elements of symmetry, can

enter into combination with each other. Compare page 14.

Correlated Forms. Obviously, by the application of hemihedrism,

tetartohedrism, and Ogdohedrism the original holohedral forms

16 INTRODUCTION.

yield two, four, or eight new correlated forms, respectively. Most

of these correlated forms are congruent and differ from each other

only in respect to their position in space. A rotation through some

definite angle is all that is necessary to have such forms occupy the

same position. Such forms are then designated as //^/sand minus,

or positive and negative, forms, page 27. Others, however, are

related to one another as is the right hand to the left, hence cannot

be superimposed and these are said to be enantiomorphous. These

are designated as right and left forms. Compare page 37.

Fig. 38. Fig. 39. Fig. 40.

M

Hemimorphism. This is a peculiar type of hemihedrism. It is

only possible upon those holohedral and hemihedral forms, or their

combinations, which possess a so-called singular** axis of symmetry.

By its application the forms occurring about one end of this axis differ

from those about the other. Such forms are hemimorphic, and the

singular axis of symmetry is said to be polar. Hence, the plane of

symmetry perpendicular to the singular axis is lost. Compare figures

38, 39, and 40.

!) An axis which occurs but once and differs from all others. For example, the axis of

tetragonal symmetry in figure 30.

.

being

OF THE 1

CUBIC SYSTEM"

Crystallographic Axes. All forms which can be referred to

three equal and perpendicular axes belong to this system. Figure 41

shows the axial cross. One axis is held

A. A.

a second extends from front to

vertically,

rear, and the third from right to left.

These axes are all interchangeable, each

designated by a. Since there are no

unknown elements of crystallization in this

system (page 9), all substances, regardless

of their chemical composition, crystalp7*

41 lizing in this system with forms having the

same parametral ratios must of necessity

possess the same interfacial angles.

Classes of Symmetry. The cubic system includes five groups

or classes of symmetry. Beginning with the class of highest symmetry,

they are:

1)

Hexoctahedral Class (Holohedrism)

2) Hextetrahedral Class \

3) Dyakisdodecahedral Class > (Hemihedrisni)

4) Pentagonal icositetrahedral Class )

5) Tetrahedral pentagonal dodecahedral Class

( Tetartohedrisrti)

Of these classes, the first three are most important, since they

possess many representatives among the minerals.

/. HEXOCTAHEDRAL CLASS.*) }\ r tt\ o\\ v

(Holohedrism.}

Elements of Symmetry, a) Planes. Forms of this class are

characterized by nine planes of symmetry. Three of these are parallel

to the planes of the crystallographic axes and, hence, perpendicular

to each other. They are the principal planes of symmetry.

They divide space into eight equal parts called octants. The six

1) Also termed the regular, isometric, tesseral, or tessular system.

2) Termed by Dana the normal group.

i

i

18 CUBIC SYSTEM.

other planes are each parallel to one of the crystallographic axes and

bisect the angles between the other two. These are termed the secondary

or common planes of symmetry. By them space

is divided

Fig.

42. Fig. 43.

into twenty-four equal parts. The nine planes together divide space

into forty-eight equal sections. These nine planes are often indicated

thus: 3 -4- 6 = 9. Figures 42 and 43 illustrate the location of the

principal and secondary planes,

respectively.

b) Axes. The intersection lines of the three principal planes

of symmetry give rise to the three principal axes of symmetry.

These are parallel to the crystallographic axes and possess tetragonal

symmetry, as illustrated by figure 44. The four axes equally inclined

Fig. 44. Fig. 45. Fig. 46.

to the crystallographic axes are of trigonal symmetry, as shown by

figure 45. There are also six axes of binary symmetry. These lie

in the principal planes of symmetry and bisect the angles ^ between

the crystallographic axes. Their location is indicated in figure 46.

These thirteen axes of symmetry may be indicated as follows:

c) Center. The forms of this class also possess this element of

symmetry. Hence, all planes have parallel counter-planes.

.

HEXOCTAHEDRAL CLASS. 19

The projection of the most general form

of this class upon a plane perpendicular to

the vertical axis, i. e., in this case a principal

plane of symmetry, shows the symmetry

relations, 1} figure 47.

FORMS.

Fig. 47.

1. Octahedron, As the name implies,

this form consists of eight

faces. Each face

is equally inclined to the crystallographic axes.

Hence, the parametral ratio may be written

(a : a

:

a), which according to Naumann and

Miller would be O and ji

i

i|, respectively.

The faces intersect at an angle of 109 28'

1 6" and in the ideal form, figure 48, are equal,

equilateral triangles.

The crystallographic axes and, hence,

the axes of tetragonal symmetry pass through

Fig. 48.

the tetrahedral angles. The four trigonal

axes join the centers of opposite faces, while

the six binary axes bisect the twelve edges.

2. Dodecahedron. This form consists

of twelve faces, each cutting two of the

crystallographic axes at the same distance,

but extending parallel to the third. The

Fig. 49.

symbols are, therefore, (a a cca), OoO, : : 1

j 10}. In the ideal form,

figure 49, each face is a rhombus and, hence, the form is often

termed the rhombic dodecahedron.

The crystallographic axes pass through the tetrahedral angles,

the trigonal axes join opposite trihedral angles, and the binary axes

the centers of opposite faces. It follows, therefore, that the faces

are parallel to the secondary planes of symmetry.

3. Hexahedron or Cube. The faces of this form cut one axis

and are parallel to the other two. This is

expressed by (a : do a

1) The heavy lines indicate edges through which principal planes of symmetry pass. The lighti

full lines show the location of the secondary planes, while dashed lines indicate the absence of planes,

3ee page 26.

20 CUBIC SYSTEM.

ooOoo, jioo}. Six such faces

are possible and when the development

is ideal, figure 50, each is a square.

The crystallographic axes pass

through the centers of the faces. The

trigonal axes of symmetry join opposite

trihedral angles, while the binary axes

bisect the twelve edges. Compare figures

Fig. 60.

Fig. 51. Fig. 52.

44, 45, and 46.

4. Trigonal trisoctahedron. 1} The faces of this form cut two

greater than /. Because the general

crystallographic axes at equal distances, the third at a greater

distance via. The coefficient

m is some rational

value greater than one

but less than infinity. The

ratio is (a a via) : : and

it

requires twenty -four

such faces to enclose

space. The Naumann

and Miller symbols are

mO, \hhl\, where h is

outline of this form is similar

to that of the octahedron, each face of which in the ideal forms is

replaced by three equal isosceles triangles,

it is termed the trigonal

trisoctahcdron, figures 51, 20 1

22 1 5,

and 52, 3O\33i\.

The crystallographic axes join opposite octahedral angles. The

trigonal axes pass through the trihedral angles and the six binary axes

bisect the twelve long edges.

5. Tetragonal trisoctahedron. 2) This form consists of twentyfour

faces, each cutting one axis at a unit's distance and the other

two at greater but equal distances ma. The value m of is, as above,

m > i < oo. The symbols are, therefore, (a

: ma :

ma), mOm,

\hll\, h > I. The ideal forms, figures 53, 2O2J2ii(, and 54,

4O4|4iiJ, bear some resemblance to the octahedron, each face of

which has been replaced by three four-sided faces, trapeziums, of

!) Also known as the trisoctahedron.

2 ) Also termed the trapezohedron, icositetrahedron, andleucitohedron.

HEXOCTAHEDRAL CLASS. 21

equal size. The form is, therefore, termed the tetrag-onal trisoctahedron.

The six tetrahedral angles 1 )

a indicate the position of

the crystallographic

axes. The trigonal

axes of symmetry join

opposite trihedral

angles, while those of

binary symmetry connect

the tetrahedral

angles 2 )

dron.

b.

6. Tetrahexahe- Fig. 53. Fig. 54.

In this form the

faces cut one axis at a unit's distance, the second at the distance

ma, where m>\< 00, and extend parallel to the third axis. The

symbols are,

(a : ma

:

therefore,

do a), oo O m,

\hko\. The twentyfour

faces in the ideal

forms, figures 55,

ooO2[2ioS, and 56,

OoO4| 41 o|, are equal

isosceles triangles.

Since this form may be Fig. 55. Fig. 56.

considered as a cube, whose faces have been replaced by tetragonal

pyramids, it is often called the pyramid cube or tetrahexahedron.

The crystallographic axes are located by the six tetrahedral

angles. The axes of trigonal symmetry pass through opposite hexahedral

angles, while the binary axes bisect the long edges.

7. Hexoctahedron.

As is indicated by -the

name, this form is bounded

by forty-eight faces.

Each cuts one crystallographic

axis at a unit's

distance, the other two at

greater but unequal dis- Fig. 57. Fig. 58.

1 ) With four equal edges.

2) These have two pairs of equal edges.

22 CUBIC SYSTEM.

tances na and ma, respectively; n is less than m, the value of m

being, as heretofore, w>i

HEXOCTAHEDRAL CLASS. 23

The relationship existing between the simple

expressed by the following diagram:

forms is well

a :

a

:

a

a : na

: ma

a : a : oo a

a :

ma

:

oo a a : oca

:

ooa

The three fixed forms are placed at the corners of the triangle

and, as is obvious, must be considered as the limiting forms of the

others. For example, the value of m in the trigonal trisoctahedron

(a a md) varies between unity and : : infinity, page 20. Hence, it

follows that the octahedron and dodecahedron are its limiting forms.

The tetragonal trisoctahedron (a

: via :

md)

similarly passes over

into the octahedron or cube, depending upon the value of m. The

limiting forms are, therefore, in every case readily recognized.

Those forms, which are on the sides of the triangle

1

^ lie in the same

zone, that is,

their intersection lines are parallel.

Combinations. The following figures illustrate some of the

combinations (page 7) of the simple forms, which are observed most

frequently.

Fig. 59. Fig. 60. Fig. 61.

Figures 59 and 60. h = oo O oo,{ioo}; o=O, {in}. Com-

1) For example, the octahedron, trigonal- trisoctahedron, and dodecahedron.

24 CUBIC SYSTEM.

monly observed on galena, PbS. In figure 59 the octahedron

predominates, whereas in figure 60 both forms are equally

developed.

Figure 61. h = 00 O oc, {100} ;

d

Cu, and fluorite, CaF 2 ,

show this combination.

= ooO, {no}. Copper,

Fig. 62. Fig. 63. Fig. 64.

Figures 62 and 63. h = ooO 00,{ 100}; o = O,{iu}; and

d -= ocO, {no}. Also observed on galena, PbS.

Figure 64. h = OoOoo,jioo|; e = OoO2, {210}. Observed

on copper, Cu; fluorite, CaF 2 ;

and

halite, NaCl.

Fig. 65. Fig. 66. Fig. 67.

Figure 65. o = O,

1 1 1 { } ;

e = 0062, J2io}. Fluorite, CaF .

d= 2

Figure 66. ooO, {no}; e = 0062, J2io}. Copper, Cu.

Figure 67. h = oo O oo,{iooj ;

i = 2O2,\2ii\. Observed on

analcite, NaAl(SiO 3) 2

.H 2 O; and argentite, Ag S. 2

303, 13"}- Spinel, MgAl O .

2 4

Figure68. o = O, {

1 1 1 } ;

*'

=

HEXOCTAHEDRAL CLASS.

Fig. 68. Fig. 69. Fig. 70.

=

Figure69 ,'= 2O2,{2ii}; O O,{in}. Argentite, S. Ag2 .

Figure 70. o =

f {in}; ^=ooO, {nof; f=2O2,{2ii

Observed on spinel, MgAl 2O 4

,

and magnetite, Fe 3

O 4

.

Fig. 71. Fig. 72. Fig. 73.

Figure 71. rf=ooO,{no};

= f 2O2,{2ii{. A common combination

observed on the garnet,

.

R'^'^SijO

Figure 72. ,'=202,{2ii{; / = |O,{332}- Garnet.

Figure 73.

d= ooO,{noJ;

5 = 3O|,J32i}. Garnet.

Figure 74.

Garnet.

rf=

Fig. 74.

o}; / = 2O2,{2ii(; ^ =

26 CUBIC SYSTEM.

2. HEXTETRAHEDRAL CLASS. 1 )

(

Tetrahedral Hemihedrism. )

Elements of Symmetry, By decreasing the elements of symmetry

of the hexoctahedral class, page 17, the other classes of the

cubic system may be deduced. In this class the principal planes of

symmetry disappear, which necessitates not only the loss of the six

axes of binary symmetry, but also the three of

Fig. 75.

tetragonal symmetry parallel to the crystallographic

axes, see page 18. The center

of symmetry also disappears. Hence, the

elements remaining are: six secondary planes

of symmetry, and four trigonal axes, which are

now polar. There are

tetrahedron.

HEXTETRAHEDRAL CLASS. 27

Each octahedron, however, yields two new correlated

forms as shown by figures 76, 77 and 78. If the shaded faces

of figure 77 are suppressed, we obtain the tetrahedron, whose

position is indicated by figure 78. However, when the shaded

faces are allowed to expand, the others being suppressed, another

tetrahedron, figure 76, similar in every respect to the first, but rotated

through an angle of 90 is obtained. These forms are, hence,

congruent and differentiated by the plus and minus signs, figure

78, plus or positive; figure 76, minus or negative. The symbols

of

the tetrahedron are written:

a: a: a O

A . O

4_

; -f

, KJIII; } ;

and K{III[.

The crystallographic

axes pass through the centers of the edges.

The axes of binary symmetry are parallel to them; those of trigonal

symmetry pass from the trihedral angles to the centers of opposite

faces.

Tetragonal tristetrahedron. From the trigonal trisoctahedron,

as shown by figures 79, 80, and 81, are obtained two congruent

forms bounded by twelve faces, which in the ideal development are

Fig. 79. Fig. 80. Fig. 81.

similar trapeziums. These forms possess a tetrahedral habit and

are called tetragonal tristetrahedrons, sometimes also deltoid

dodecahedrons or simply deltoids.

The symbols are:

a: a: ma mO ,

7> f

mO

-f- ; -f , K\hhl\ (figure 80; ,

*\hhl\

(figure 79).

1) The letfer K (KA.O/OS, inclined) is placed before the Miller indices of forms of this class

because their faces are inclined. This type of hemihedrism is often known as the inclined-face

hemihedrism.

mQm

28 CUBIC SYSTEM.

The crystallographic axes pass through opposite tetrahedral

angles, while the axes of trigonal symmetry join opposite trihedral

angles, one of which is acute, the other obtuse.

Trigonal tristetrahedron. The application of the tetrahedral

hemihedrism to the tetragonal trisoctahedron produces two congruent

half-forms, bounded by twelve similar isosceles triangles, figures*

82, 83, and 84. Since these new forms may be considered as

tetrahedrons whose faces have been replaced by trigonal

pyramids, they are termed trigonal tristetrahedrons^ or pyramid

tetrahedrons. Sometimes, moreover, the term trigonal

dodecahedron is also used.

Fig. 82. Fig. 83. Fig. 84.

The symbols are written:

mOm -.

a \ma\ma

,

+/ + -T-T-5 -T~> {A//} (figure 84);- -j-, {*//}

(figure 82).

The crystallographic axes bisect the long edges. The trigonal

axes pass from the trihedral angles to the opposite hexahedral.

Hextetrahedron.

In precisely the same manner the hexoctahedron,

figure 86, yields two congruent forms of tetrahedral habit,

bounded by twenty-four similar scalene triangles. These new forms

are called hextetrahedrons.

*) The following relationship between this and the preceding form and their respective

holohedral forms should be carefully noted, viz: The trigonal trisoct?hedron (each face is triangular)

yields the tetragonal tristetrahedron (faces of tetragonal outline), wh'le, vice versa, the tetragonal

trisoctahedron furnishes the trigonal tristetrahedron. Compare figures 79 to 84.

HEXTETRAHEDRAL CLASS. 29

Fig. 85.

The symbols are:

a \na\ma mQn

\hkl\ (figure 87); - hkl\

(figure 85.)

The crystallographic axes connect opposite tetrahedral angles.

The trigonal axes of symmetry pass through opposite hexahedral

angles, one of which is more obtuse than the other.

Hexahedron, dodecahedron, and tetrahexahedron. As is

evident from figure 7 5, no forms, geometrically new, can result from

the application of this type of hemihedrism on the cube, dodecahedron,

and tetrahexahedron. The faces of these forms belong simultaneously

to different octants and, hence, the suppression of a portion

of a face in one octant is counterbalanced by a corresponding

expansion in another. Therefore, no change in these forms can

result. They are from a geometrical standpoint exactly similar to

those of the hexoctahedral class. Their symmetry is, however, of a

lower grade. This is not to be recognized on models. On crystals,

however, the form and position of the so-called etch figures, as also

the different physical characteristics of the faces, reveal the lower

grade of symmetry 1 ). These forms are, therefore, only apparently

holohedral.

!) When crystals are subjected to the action of some solvent for a short time, small

depressions or elevations, the so-called etch figures, appear. Being dependent upon the internal

molecular structure, their form and position indicate the symmetry of the crystal. For instance, figure

88 shows the etch figures on a crystal (cube) of halite,

NaCl. Here, it is evident, that the symmetry of the

figures in respect to that of the cube is such as to

place the crystal in the hexoctahedral class. Figure

81) represents a cube of sylvite, KC1, which geometrically

does not differ from the crystal of halite. A

lower grade of symmetry is, however, revealed by

the position of the etch figures. This crystal belongs

to the pentagonal icositetrahedral class, page 36, for

no planes of symmetry can be passed through these

Fig gg^

30 CUBIC SYSTEM.

The following table shows the important

of this class of symmetry.

features of the forms

figures, which at the same time are planes of

symmetry of the cube, as is the case with the

crystal of halite, figure 88. Fora fuller discussion

of these interesting figures consult Groth, Physikalische

Krystallographie, 4te Auflage, 1905, 251;

also Dana, Text-book of Mineralogy, 1898, 149.

Figures 90 and 91 show two cubes representing

crystals of sphalerite, ZnS (figure 90), and

pyrite, FeS2 (figure 91). Although these form?

Fig. 90. Fig. 91. do not differ from the holohedral, it is at once seen

HEXTETRAHEDRAL CLASS. 31

Combinations. Some of the more common combinations are

illustrated by the following figures:

Fig. 92. Fig. 93. Fig. 94.

O

Figure 92. o =

-\ , KJIIIJ; h = OoO 00, K| iooj. Observed

on sphalerite, ZnS.

Figure 93. o = + ,

Sphalerite.

*{ 1 11 o' = -

} ; , K{III(.

2

O

Figure 94. 0=+, "Jin!; h = ooO oo, *{ ioo[ ;

d

00 O, K{IIO{. Tetrahedrite (Cu 2 , Fe, Zn) 4 (As, Sb) 2 S 7 .

Figure 95. o ~- -h ,

Tetrahedrite.

O

=

-

2O2

- ie2ii-.

Fig. 95.

2O2

Figure 96. n = +

,

Fig. 96. Fig. 97.

r =

ooO,

Tetrahedrite.

that adjoining faces possess striations extending in different directions. Figure 90 possesses six

secondary planes of symmetry, the principal are wanting, and, hence this cube is only apparently

holohedral. It belongs to hextetrahedral class. Figure 91 possesses a still lower grade of symmetry

for here only three principal planes are present, and it must, therefore, be referred to the

dyakisdodecahedral class, page 32,

c O

"^SSS

1 !*

This combination occurs on boracite, Mg 7 Cl 2B 16

O 30

.

32 CUBIC SYSTEM.

Figure 97. d ooO, K{IIO|; m-

,KJ3iiJ.

Sphalerite.

Figure 98. /i=ooOoc, K{IOO|; o

+ ,

O

K\\\\

o

;

d

Fig. 98.

=

z; =

3. DYAKISDODECAHEDRAL CLASSY

(^Pyritohedral Hemihedrism.}

Fig. 99.

Elements of Symmetry. Here the six secondary planes and

the six axes of binary symmetry are lost. The

elements of symmetry which remain are, therefore,

three principal planes parallel to the

planes of the crystallographic axes, four

trigonal axes, and also the center of symmetry.

The three axes parallel to the crystallographic

axes now possess binary symmetry. Figure 99

shows these elements as well as the application

of the hemihedrism, which will be discussed

in the next paragraph.

Pyritohedral hemihedrism 2 . In this class the forms may be

assumed as derived from the holohedral types by the expansion of

the faces lying wholly within alternate spaces formed by the

intersection of the secondary planes of symmetry, page 18. Such

1) Called by Dana the pyritohedral group.

2) Also termed pentagonal or parallel-face hemihedrism, having reference to the pentagonal

outline and parallel arrangement of the faces, respectively.

DYAKISDODECAHEDRAL CLASS. 33

faces or pairs of faces are then symmetrical to the three principal

planes of symmetry, figure 99.

Pyritohedron. The application of this type of hemihedrism to

the tetrahexahedron, figure 101, produces two correlated, congruent,

hemihedral forms, figures 100 and 102, bounded by twelve similar

faces. Each face is an unequilateral pentagon, four sides of which

are equal. Since these forms are congruent, a rotation through 90

is all that is necessary to bring them into precisely the same position

in space. They are, hence, designated as 1}

plus and minus forms.

Fig. 100.

Fig. 101. Fig. 102.

The symbols are:

fa:ma:aca'}

ma\ do a f ocOral

| -J- J; +| -J- J,

TJA0} (figure 102);

(figure 100).

Because this form occurs frequently on pyrite it is termed the

pyritohedron, although pentagonal dodecahedron^ is quite often

used.

The axes of binary symmetry, hence, also the crystallographic

axes bisect the six long edges. The trigonal axes pass through the

trihedral angles, the edges of which are of equal lengths.

1) Also designated as right and left. It is preferable, however, to use those terms in reference

to enantiomorphous forms only, page 16.

2) In this class, TT (TrapoAAryAos, parallel faced) is placed before the Miller indices, see page

27. To distinguish the other symbols from those of the preceding class, they are enclosed in brackets.

3 ) The regular pentagonal dodecahedron of geometry, bounded by equilateral pentagons

intersecting in equal edges and angles is crystallographically an impossible form, the value of m being

which is irrational, compare page 10.

^4

CUBIC SYSTEM.

Dyakisdodecahedron. By the expansion and suppression of alternate

pairs of faces crossed by the principal planes of symmetry, the

hexoctahedron, figure 104, yields two correlated, congruent forms,

each bounded by twenty-four similar trapeziums, figures 103 and 105.

These forms are the dyakisdodecahedrons also

%

termed didodecahedrons,

or diploids.

Fig. 103. Fig. 104. Fig. 105.

The symbols are

\a:na:ma --

|_ 2

' -\ hkl \ (figure 105):

mOn

ir\hlk\ (figure 103).

The crystallographic axes, also those of binary symmetry, pass

through the six tetrahedral angles possessing two pairs of equal edges.

The trigonal axes join opposite trihedral angles.

Other Forms. The hexahedron, octahedron, dodecahedron,

trigonal trisoctahedron, and tetragonal trisoctahedron, the other

forms of the holohedral type, do not yield new forms by the application

of this hemihedrism. This is clearly shown by figure 99, illustrating

the elements of symmetry of this class. Being apparently

holohedral, these forms may occur independently or in combination,

but always with the full number of faces. Their symmetry is, however,

less than that of the holohedrons. See page 29.

In the following table -the important

this class are indicated.

features of the forms of

DYAKISDODECAHEDRAL CLASS. 35

Combinations.

The accompanying figures show some combinations

of the forms of this class.

Fig. 106.

Figure 1 06. h = ocO oo, v\ 100} ;

Commonly observed on pyrite, FeS 2

.

Figures 107 and 108. o = O, ir\

i 1 1 \ ; +

1 g J, 7r2iOi

,

the

36 CUBIC SYSTEM.

In figure 107 the octahedron predominates, whereas in figure 108

both forms are about equally developed.

Pyrite.

Fig. 109. Fig. 110. Fig. 111.

Figure 109. h =ooOoo, TrjiooJ; 5 = + I ^M,

w|32i|.

Pyrite.

Figure no. e= -f I, 7r|2ioS; o = O, TT{III\.

Between o and e but in the same zone, -M I ^SS 21 1- Pyrite.

Figure in. ^ = ooOoo, TT\\QQ\\ o = O, TT|

1 1 1 1 ;

e =

[ooO2l I 7r|2io|. Cobaltite, CoAsS.

4. PENTAGONAL ICOSITETRAHBDRAL CLASS. 1 )

( Plagihedral or Gyroidal Hemihedrism. )

Elements of Symmetry. All planes, as well as the center of

symmetry, are lost. There

Fig. 112.

intersection of the nine planes of symmetry,

page 1 8. Compare figure 112.

Termed by Dana the plagihedral group.

remain, however, all of the thirteen axes,

namely, three tetragonal, four trigonal, and

six binary axes. Figure 112 shows these

elements and also the method of the application

of the plagihedral hemihedrism.

Plagihedral Hemihedrism. Forms of

this class may be assumed as derived from

the holohedrons by the alternate expansion

and suppression of faces lying wholly within

each of the forty-eight sections, resulting from

PENTAGONAL ICOSITETRAHEDRAL CLASS. 37

Pentagonal Icositetrahedron. By the extension and suppression,

respectively, of alternate faces of the hexoctahedron, figure 114,

two new correlated forms, bounded by twenty-four equal unsymmetrical

pentagons result. *

These forms are termed pentagonal icositetrahedrons

or gyroids. They are not congruent, for they cannot be

brought into the same position by rotation and, hence, are not

superimposable. Therefore, they are enantiomorphous, page 16,

and distinguished as right, figure 115, and left, figure 113, according

to which of the top faces (right or left) in the front upper octant

has been extended.

Fig. 113.

Fig. 114. Fig. 115.

The symbols are:

mOn

a: na : ma

r.l- -\r -- *

mOn

The crystallographic axes, also those of tetragonal symmetry,

join opposite tetrahedral angles. The trigonal axes pass through

those trihedral angles which possess equal edges, while the six binary

axes bisect the twelve edges intermediate between those forming the

tetrahedral angles.

Other forms. ^Jhe

six other holohedrons are not from a geometrical

standpoint effected by this hemihedrism. A study of figure

112 shows that no new forms can result, for on these holohedrons

none of the faces lie wholly within one of the forty- eight sections

referred to on page 36. The octahedron, dodecahedron, hexahedron,

the trigonal and tetragonal trisoctahedrons, and the tetrahexahedron

are only apparently holohedral.

i) In this class,

y (yvpos, bent) is placed before the Miller indices. Compare footnotes on

pages 27 and 33.

38 CUBIC SYSTEM.

The principal features of the forms of this class may

as follows:

be tabulated

Combinations. Figure 116. 2=202,

m

=/ Sal y\2ii\ t

.s ~>y{%75l- Ammoniac,

NH 4 C1.

5. TBTRAHEDRAL PENTAGONAL DODECAHE-

DRAL CLASSY

( Tetartohedrism. )

Fig. 116. Elements of Symmetry. The nine

and the six

planes, the three axes of tetragonal of binary symmetry, as also the center, are lost. The elements of

this class are, hence, four polar axes of trigonal and three of binary

1) The tetartohedral group of Dana.

TETRAHEDRAL PENTAGONAL DODECAHEDRAL CLASS. 39

symmetry, the latter being parallel

crystallographic axes. See figure 117.

to the

Tetartohedrism. The simple tetartohedral

forms may be conceived as derived from

the hemihedrons of any one of the three

hemihedral classes tetrahedral, pyritohedral,

or plagihedral by the subsequent application

of one of the other two methods. Th^

result is in each case the same. Compare

figures 118, 119, 120, 122, and 125.

Fig. 117.

Fig. 121. Fig. 122. Fig. 123.

Fig. 124. Fig. 125.

Fig. 126.

Tetrahedral pentagonal dodecahedron. From the hexoctahedron

by the successive application of two types of hemihedrism four

40 CUBIC SYSTEM.

new forms of tetrahedral habit, bounded by twelve unsymmetrical

pentagons, result. The derivation of these forms is easily to be seen

from figures 121-126, also figure 37, page 15. In figure 122,

the form derived by the expansion of the unshaded faces is known as

the left positive tetrahedral pentagonal dodecahedron, whereas

the one derived from the shaded faces alternating with these i. e.,

in the same octant is the rig-Jit positive form. From figure 125

the left negative and rig-Jit negative forms are likewise possible.

a\ na\ ma

7

The symbols according to Weiss are -r r, - I .

4

According to Naumann and Miller they may be written:

1. -\- r - -, Kir\khl\*\ Positive right, figure 123.

tilOn

2. r - , KTr\hkl\, Negative rigJit, figure 126.

4

3. -f- /- ,

4. -/-

,

4

KTr\hklt \,

Positive left, figure 121.

KTr\khl\, Negative left, figure 124.

Forms i and 2, also 3 and 4, are among themselves congruent,

whereas the pairs I and 3, and 2 and 4, are enantiomorphous.

The crystallographic axes bisect the six equal edges, while the

four trigonal axes join opposite trihedral angles of which one is more

obtuse than the other. These trihedral angles possess equal edges.

Other forms.

If tetartohedrism be applied to the other holohedrons,

it follows that four of them will yield forms, as follows:

Octahedron two tetrahedrons, figures 76 and 78, page 26.

Trigonal trisoctahedron two tetragonal tristetrahedrons, figures

79 and 81, page 27.

Tetragonal trisoctahedron

82 and 84, page 28.

two trigonal tristetrahedrons, figures

Tetrahexahedron two pyritohedroris, figures 100 and 102,

page 33-

The first three forms do not differ geometrically from those

obtained by the tetrahedral hemihedrism, while the fourth is the same

as that derived by the pyritohedral hemihedrism. They are, hence,

i) Two letters, each representing one of the types of hemihedrism applied, are used with the

Miller indices in this class.

TETRAHEDRAL PENTAGONAL DODECAHEDRAL CLASS. 41

only apparently hemihedral forms.

The cube and dodecahedron are

unchanged geometrically and, therefore, apparently holohedral.

The following table shows the principal features of the forms of

this class:

1 ) One set is more obtuse than the other.

ooO

42 CUBIC SYSTEM.

Combinations. In this class it is evident that the apparently

holohedral and hemihedral forms of the various classes, as described

on pages 40 and 41, may

occur together on the same

crystal. For example,

figures 127 and 128 show

crystals of sodium chlorate,

Fig. 127.

Fig. 128.

NaClO 3

, where h = 00 O oo,

= OCO, KIT 10

O

K7T |

I I I

(figure 127) = - [ ^- 2 ],

{ I20} p .

(figure

I2g)= + F GC021

\ " ^*

Fig. 129.

Fig. 130.

Fig. 131.

R rtsrn N A I3 and ' ISI illustrate crystals of barium nitrate,

Ba(N0 3 ) 2 , with the following forms: h = --

X=

--. w ir7Tl.^_ T^02

I

{!{;#=

2

oo, KTTJ ioo; ;

o =

-^-|, T-'l

W jI20|;

'

HEXAGONAL SYSTEM.

Crystallographic Axes. This system includes all forms which

can be referred to four axes, three of which are equal and lie in a

horizontal plane, and intersect each other

at an angle of 60. These are termed the

-c

Fig. 132.

secondary or lateral axes, being designated

by the letter a. These axes are interchangeable.

The fourth, a principal axis,

is

perpendicular to the plane of the secondary

axes and is termed the c axis. It may

be longer or shorter than the secondary

axes. The three equal axes, which bisect

the angles between the secondary axes,

are

the intermediate axes. These may be

designated by b. Figure 132 shows an axial

cross of this system.

In reading crystals of the hexagonal system, it is customary to

hold the c axis vertical, letting one of the secondary or a axes extend

from right to left. The extremities of the secondary axes are

alternately characterized as plus and minus, see figure 132. In

referring a .form to the crystallographic axes, it is common practice

to consider them in the following order: # t first, then a 2 , thirdly 3 ,

and lastly the c axis. The symbols always refer to them in this

order. It is also to be noted that in following this order, one of the

lateral axis will always be preceded by a minus sign.

*

Since the lengths of the a and c axes differ, it is

necessary to

assume for each substance crystallizing

in this system a fundamental

form, whose intercepts are taken as representing the unit lengths of

the secondary and principal axes, respectively. The ratio, which

exists between the lengths of these axes is called the axial ratio and

is

always an irrational value, the a axis being assumed as unity,

page ;



44 HEXAGONAL SYSTEM.

Classes of Symmetry.

The hexagonal system includes a larger

number of classes of symmetry than any other system, namely,

twelve. The order in which they will be discussed is as follows:

tt

t *

t*

i.

2.

3-

4-

5-

6.

7-

8.

9-

10.

ii.

Dihexagonal bipyramidal class

Dihexagonal pyramidal class

Ditrigonal bipyramidal class

Ditrigonal scalenohedral class

Hexagonal bipyramidal class

Hexagonal trapezohedral class

Ditrigonal pyramidal class

Hexagonal pyramidal class

Trigonal bipyramidal class

Trigonal trapezohedral class

Trigonal rhombohedral class

12. Trigonal pyramidal class

( Holohedrism}.

f Holohedrism and\

\hemimorphism.

( Hemihedrism).

(Hemihedrism and\

\hemimorphism.

( Tetartohedrism.)

Tetartohedrism

and hemimorphism

( Ogdohedrism).

Those classes marked with an * are the most important, for

nearly all of the crystals of this system belong to some one of them.

No representatives have as yet been observed for the classes marked

by t. Those marked % are often grouped together and form the

trigonal system.

Symmetry,

/. DIHEXAQONAL BIPYRAMIDAL CLASS.U

of any in the hexagonal system.

(Holohedrism.}

This class possesses the highest grade of symmetry

a) Planes. In all there are seven planes of symmetry. One of

these, the -principal plane, is parallel to the plane of the secondary

axes, hence, horizontal. The other planes are divided into two

series of three each, which are termed the secondary and intermediate,

respectively. Each of the secondary planes includes the c

or principal axis and one of the secondary, a, axes. These planes

are, therefore, vertical and perpendicular to the principal plane.

The normalgroup of Dana.

j

J

DIHEXAGONAL BIPYKAMIDAL CLASS. 45

They intersect at angles of 60. The intermediate

planes are also vertical and perpendicular

to the principal plane^, for they

bisect the angles between the secondary

planes and, hence, each includes the.c and

one of the intermediate axes.

The secondary and principal planes

divide space into twelve equal parts, called

dodecants; the seven planes, however, into

twenty-four parts, figure 133.

These planes are often designated as

follows:

Fig. 133.

i

Principal -f- 3 Secondary -f 3 Intermediate = 7 Plants.

b) Axes. Parallel to the vertical or c axis is an axis of

hexagonal symmetry, while the axes parallel to the secondary and

intermediate axes possess binary symmetry. These axes are often

indicated, thus,

i*+3-h3

= 7 axes.

c) Center. This element of symmetry is also present, requiring

every face to have a parallel counter-face. Figure 134, the

projection of the most complicated form

upon a plane perpendicular to the vertical

axis, shows the elements of symmetry of

this class.

i.

Hexagonal bipyramid of the first

order. From figure 132, it is obvious that

any plane which cuts any two adjacent

secondary axes at the unit distance from

the center must extend parallel to the

Fig 134

third. If such a plane be assumed to cut

the c axis at its unit length from the center, the parametral ratio

would then be

According to the above elements of symmetry, twelve planes

possessing this ratio are possible. They enclose space and give rise

to the form termed the hexagonal bipyramid^ of the first order,

1) Since these are really double pyramids, the term bipyramid is employed.

Fig. 136. Fig. 137.

46 HEXAGONAL SYSTEM.

Fig. 135. but intercept the c axis at the distance mc^

the coefficient m being some rational value

figure 135. In the ideal form, the faces are

all equal, isosceles triangles. The symbols

are (aiOOa: a: c), P, jionf. 1 )

Because the

intercepts along the c and two secondary axes

are taken as units, such bipyramids are also

known as fundamental or unit bipyramids,

page 6.

Planes are, however, possible which cut

the two secondary axes at the unit distances,

smaller or greater than I, see page 6. Such bipyramids, according

as m is greater or less than unity, are more acute or obtuse than

the fundamental form. They are termed modified hexagonal bipyramids

of the first order. Their symbols are (a: oca: a:mc), mP,

\h o hl\, where m = y,

also m > o < oc .

The principal axis passes through the hexahedral angles, the

secondary axes join tetrahedral angles, while the intermediate bisect

the horizontal edges. Hence when such bipyramids are held correctly,

a face is directed towards the observer. The various axes of

symmetry are located by means of the above.

2.

Hexagonal bipyramid of the second order. In form, this

bipyramid does not differ from the preceding. It is, however,

i) In this system it is advantageous to employ the indices as modified by Bravais (h ikl) rather

than those of Miller, who uses but three.

DIHEXAGONAL BIPYRAMIDAL CLASS. 47

to be distinguished by its position in respect to the secondary axes.

The bipyramid of the second order is so held that an edge, and not a

face, is directed towards the observer. This means that the secondary

axes are perpendicular to and bisect the horizontal edges as shown

in figure 136. Figure 137 shows the cross section including the secondary

axes. From these figures it is obvious that each face cuts one

of the secondary axes at a unit distance, the other two at greater but

equal distances. For example, AB cuts a z

at the unit distance OS,

and a l

and a at 2 greater but equal distances OM and ON, respectively.

The following considerations will determine the length of OM

and ON, the intercepts on a l

and 2 ,

in terms of OS = i.

As already indicated, the secondary axes are perpendicular to the

horizontal edges, hence OS and ON are perpendicular to AB and BC,

respectively. Therefore, in the right triangleSpRB

and NRB, the

side RB is common and the angles OBR and NBR are equal.

1}

Therefore, OR == RN. But OR = OS == i.

Hence, ON = OR + RN == 2.

In the same manner it can be shown that the intercept on a^

is equal to that along 2 , that is, twice the unit length. The

parametral ratio of the hexagonal bipyramid of the second order,

therefore, is

(20: 2a: a: mc\ or expressed according

to Naumann and

2/1

Bravais, mP2 and \hh2h l\, where -j-

= m. -Figure 137 shows

the positions of the bipyramids of both orders in respect to the

secondary axes, the inner outline representing that of first, the outer

the one of the second order.

Fig. 138.

i) For, angle ABC equals 120, angle NBR is then 60, being the supplement of ABC. But

the intermediate axis OZ bisects the angle ABC, hence angle OBR is also 60.

.

48 HEXAGONAL SYSTEM.

3. Dihexagonal bipyramid. The faces of this form cut the

three secondary axes at unequal distances. For example, in figure

138 the face represented by dB cuts the a^ axis at A, 2 at C, and

a s

at B. Assuming the shortest of these intercepts as unity, hence,

OB = a i, we at once see that one of these axes is cut at a unit's

distance from O, the other two, however, at greater distances.

If we

let the intercepts ,OA and OC be represented by n(OB) = na, and

= />(OB) pa, respectively, the ratio will read

na :pa

: a :

me, mPn, \hikl\.

n

In this ratio p

Twenty-four planes having this ratio

are possible and give rise to the form called

the dihexag'onal bipyramid, figure 139.

In the ideal form the faces are equal,

scalene triangles, cutting in twenty-four

polar 2) ,

a and b, and twelve equal basa! 3)

edges. The polar edges and angles are

alternately dissimilar. This is shown by

figure 140, where the heavy inner outline

represents the form of the first order, the

outer the one of the second, and the intermediate

outlines the dihexagonal type Fig. 139. in

respect to the secondary axes.

i) From the above discussion, it follows that in figure 138

OA:OC: OB = :/:!.

Draw XB parallel to a 2 .

and then

OA:XA = OC:XB.

But the triangle OXB is equilateral,

Hence, XB = XO = OB = 1.

And XA = OA OX = OA 1.

Therefore, OA : OA 1 = OC : 1.

But OA = n, and OC =/,

Hence, w:n !=/:!,

z4ro,

r

^l = p -

It can also be shown that the algebraic sum of the Miller- Bravais indices -{

hik } is equal to

h + i + ~k = o.

For, OA = -4-

n

OC = 4^ and OB

1

Therefore, -T-: =- r~ = 7-

:

r-,

h ' h ~~ k

J_. J_

1

t

-i-> page 12.

Or, k = h + 1.

Hence, h -\- i + k = o.

Those joining the horizontal and principal axes.

These lie in the principal plane of symmetry.

DIHEXAGONAL BIPYRAMIDAL CLASS. 49

These three hexagonal bipyramids are closely related, for, if we

suppose the plane represented by AB, figure 140, to be rotated about

the point B so that the intercept along a 2

increases in length, the one

Fig. 140.

along j decreases until it equals oB' = oB = i. Then the plane is

parallel to a and the ratio for the 2

bipyramid of the first order results.

If, however, AB is rotated so that the intercept along a 2

is decreased

in length, the one along a^ increases until it equals oC = 2oB' = 2a.

When this is the case, the intercept on 2

is also equal to 2 i < 2, and/ > 2 < 00.

The dihexagonal bipyramid whose polar edges and angles are all

equal is crystallographically not a possible form, because the value of

n would then be ^(i + 1/3)

= 1/2. sin 75

= 1.36603+, which of

course is irrational. It also follows that in those dihexagonal bipyramids,

where the value of n is less than 1.36603 + for , instance,

t = i. 20, the more acute pole angles indicate the location of the

secondary axes, the more obtuse that of the intermediate, and vice

50 HEXAGONAL SYSTEM.

versa, when n is greater than 1.36603 + for , example, |-=i.6o.

This is clearly shown by figure 140.

Hexagonal prism of the first order. This form is easily derived

from the bipyramid of the same order by allowing the intercept

Fig, 141.

along

the c axis to assume its maximum

value, infinity. Then the twelve planes of

the bipyramid are reduced to six, each

plane cutting two secondary axes at the unit

distance and extending parallel to the c

:

axis. The symbols are (a

: oca a: oor),

OoP, |ioio|. This form cannot enclose

space and, hence, may be termed an open

form, page 6. It cannot occur independently

and is always

to be observed in

combination, figure 141. The secondary

axes join opposite edges,

i. e., a face is

directed towards the observer when properly

held.

Hexagonal prism of the second order.

This prism bears the same relation to the

preceding form that the bipyramid of the

second order does to the one of the first,

Fig. 142.

page 46. The symbols are (2a:2a :a : 00 ^),

00 P2, jii2o[. It is, hence, an open form

consisting of six faces. The secondary axes

join the centers of opposite faces, hence,

an edge

is directed towards the observer,

figure 142.

Fig. 143.

Dihexagonal prism. This form may

be obtained from the corresponding bipyramid

by increasing the value of m to infinity,

which gives (na

:

pa

:

a :

ocr), OoPw,

\hiko\. This prism consist of twelve

faces whose alternate intersection angles are

dissimilar.

This form, figure 143, is closely

related to the corresponding bipyramid and,

hence, all that has been said concerning

DIHEXAGONAL BIPYRAMIDAL CLASS. 51

the dihexagonal bipyramid, page 48, in respect

to the location of

the secondary axes and its limiting forms might be repeated here,

substituting, of course, for the bipyramids of the first and second

orders the corresponding prisms.

7. Hexagonal basal pinacoid. The faces of this form are

parallel to the principal plane of symmetry and possess the following

symbols (cca oca 0/oa: c), OP, joooij. It is evident from the

: :

presence of a center and principal plane of symmetry that two such

planes are possible. This, like the prisms, is an open form and must

always occur in combination. Figure 141 shows this form in combination

with the prism of the first order.

These are the seven simple forms possible in this system.

principal features may be summarized as follows:

Their

I

52 HEXAGONAL SYSTEM.

Relation of forms. The following diagram, similar to the one

for the cubic system, page 23, expresses very clearly the relationship

existing between the various simple forms .

000 ; oca : ooa : c

a: ooa : a :

na :

pa

:

a : me

a : ooa : a : ooc-

-na :

pa

:

:a : ace- 2a : 2a

a

:

ooc

Combinations. The following figures illustrate some of the

combinations of forms of this class.

Figure 144,^ = P, icTi

{ } ;

o = mP, \holi l\.

Figure 145, p = P, j loir}; n = P2 {1121}.

Fig. 144. Fig. 145. Fig. 146.

Figure 146, p = P, { 101 1 } ; p

= |P 2, 12243^.

Figure 147, m = ooP, \\oio] ;p = P, {ion}.

Figure 148, m = ooP,

Jioio}; p = P, jioii}; u =

2P, {2021} ;

c = OP, {

oooi |;

s = 2P2; jii2i}; and v =

3 P|, 52131}. This combination

occurs on beryl, Be 3

Al 2

(Si0 3 ),

DIHEXAGONAL PYRAMIDAL CLASS. 53

2. DIHEXAGONAL PYRAMIDAL

CLASS.v

(Holohedrism with Hetnimorphism.}

Fig 147. Fig. 148.

Symmetry. The forms of this class are hemimorphic, that is,

the principal plane of symmetry disappears and

the singular, c y

axis is now polar, page 16.

The disappearance of the principal plane

necessitates also

the loss of the center and six

binary axes of symmetry. Hence, the remaining

elements are three secondary and three

intermediate planes, and one polar axis of

hexagonal symmetry parallel

to the c axis.

Figure 149 shows the elements of symmetry

of this class. 2)

Forms. The forms of this class differ from those of the

preceding (holohedral) in that the faces occurring

Fig. 149.

pole 3) are to be considered as belonging to independent forms.

Hence, each of the three bipyramids yields two new forms, called

upper and lower pyramids, respectively. For example, the dihexa-

Fig. 150. Fig. 151. Fig. 152.

1 ) Hemimorphic group of Dana .

2) The heavy dotted and dashed line not only indicates the absence of the principal plane but

also shows that hemimorpbism is effective. Compare pages 26, 32, and 36.

8 ) The ends of the principal or c axis are often spoken of as poles.

54 HEXAGONAL SYSTEM.

gonal bipyramid yields the upper and lower dihexagonal pyramids, 1}

each possessing twelve faces. Figures 150, 151, and 152 show the

upper forms of the three bipyramids. These pyramids are open

forms. They are shown in combination with the lower basal

pinacoid, for it is also divided into an tipper and lozuer form of one

face each. The symbols of these forms are the same as those used

for the holohedral, except that the end of the c axis is indicated

about which they occur. Since, however, the development of the

prisms is the same about both poles, no new forms result from them.

The principal features and symbols of the forms of this class are

given in the following table:

1) The term pyramid in itself suggests hemimorphism, since it is not a doubly terminated form

as is the bipyramid.

Combinations.

OP

Figure 153,

56 HEXAGONAL SYSTEM.

d) Trapezohedral hemihedrism. All planes of symmetry

possible in this system divide space into twenty-four sections. The

extension of faces occurs in alternate sections of this character,

figure 158.

Of these

hemihedrisms, the rhombohedral and pyramidal types

are the most important. No representative of the trigonal

hemihedrism has yet been observed.

3. DITRIOONAL BIPYRAMIDAL CLASS.

( Trigonal Hemihedrism.}

Symmetry. From figure 155 showing this method of hemihedrism

it is obvious that the secondary

planes of symmetry are lost. With them the

center and the axis of hexagonal symmetry

also disappear. The elements of this class

are, hence, one principal and three intermediate

planes, three binary axes parallel to the

intermediate, and an axis of trigonal symmetry

parallel to the c axis. The binary axes are

polar. Figure 159 not only shows these

Fig. 159. elements but the application of the hemihedrism

as well.

Trigonal bipyramids. From the hexagonal bipyramid

of the

first order two correlated, congruent forms, each bounded by six

equal isosceles triangles, result. These forms and their position in

respect to the secondary axes are shown by figures 160-165. They

, a: 00 a: a: me

are the trigonal bipyramids. The symbols are j

mP

hohl\i figure 162; , \ohhl\, figure 160.

- 2 2

The axis joining the trihedral angles is of one of trigonal

symmetry, those passing through the centers of the horizontal edges

to the opposite tetrahedral angles are of binary symmetry. These

are parallel to the intermediate axes.

Trigonal prisms. The corresponding hexagonal prism yields

two trigonal prisms,

1}

each bounded by three faces, as is shown by

figures 163

to 168.

Being open forms, they are shown in combination with the basal pinacoid.

,

a:

DITRIGONAL BIPYRAMIDAL CLASS. 57

Fig. 160.

Fig. 161. Fig. 162.

Fig. 165.

Fig. 163.

Fig. 166.

Fig. 167. Fig. 168.

The symbols are :

OOP

figure 1 68; ohho\, figure 166.

oca: a: oo^l ooP -

,

\hoho\,

+ I- I! +

-

The trigonal axis is parallel to the intersection lines of the prism

faces, while those of binary symmetry pass from the centers of the

faces to those of the opposite edges, figures 166 and 168.

Ditrigonal bipyramids.

Every dihexagonal bipyramid, when

subjected to the trigonal hemihedrism, gives rise to two correlated

and congruent forms, bounded by twelve scalene triangles, which are

58 HEXAGONAL SYSTEM.

known as the ditrig'onal bipyramids.

of these forms are illustrated by figures 169 to 174.

:

_, :

\na pa a :

The me] symbols are: +_

,

-y-

in P n .

.

171; , \ihkl\, figure 169.

The derivation and position

mPn

-| ,

\hikl\, figure

The trigonal axis joins the hexahedral angles, those of binary

symmetry extend from an obtuse to an opposite more acute tetrahedral

angleḞig.

172.

I

I

j_-

Fig. 175. Fig. 176. Fig. 177.

DITRIGONAL BIPYRAMIDAL CLASS. 59

Ditrigonal prisms. The dihexagonal prism yields two ditrigonal

prisms, as shown by figures 172 to 177. The symbols are

[na:pa\a\ oo^l ocP;; mPn

,

+ \hiko\, figure 177; , \ihko\

2

j

-^

,

figure 175.

The trigonal axis is parallel to the intersection lines of the prism

faces, those of binary symmetry are parallel to the intermediate axes.

Other forms.

The bipyramids and prism of the second order as

also the basal pinacoid are not changed geometrically by the trigonal

hemihedrism, for none of their faces lie wholly within the sections

formed by the secondary axes. Compare figures 159 and 164. These

forms are, therefore, apparently holohedral.

No representative of this class has yet been discovered.

The chief characteristic of the forms may be tabulated as follows:

60 HEXAGONAL SYSTEM.

4. D1TRIQONAL SCALENOHEDRAL CLASS.*)

(Rhombohedral ffemihedrism.}

Fig. 178.

Symmetry.

The principal and secondary

planes of symmetry together with the

hexagonal axis are lost. The following

elements are present: three intermediate

planes, three axes of binary and one of

trigonal symmetry,

also the center. Figure

178 shows these elements and the application

of the rhombohedral hemihedrism,

page 55.

Rhombohedrons. From the hexagonal bipyramid

order two new congruent forms are the result of this type of

of the first

hemihedrism,

figures 181 to 183. In the ideal development each of these

forms is bounded by six equal rhombs and are called positive and

negative rhombohedrons. The lateral

edges form a zigzag line about the torm.

The six polar edges form two equal trihedral

angles, bounded by equal edges.

or smaller than the

These may be larger

other trihedral angles, according to the

value of a:c. 2 ^

i) Dana terms this

class the rhombohedral

Fig. 179.

Fig. 180.

would be 1 :

T/1.5

= 1 :

1.2247+.

2) The cube, when

held so that one of its axes

of trigonal symmetry, page

IS, is vertical, may be considered

as a rhombohedron

whose edges and

angles are equal. "The

ratio, a :

c, in this case

Those rhombohedrons, therefore,

whose c axes have a greater value than 1.2247+ have

pole angles less than 90. When, however, the value is less than

1.2217+, the pole angles are then greater than 90 and, hence,

such rhombohedrons may be spoken of as acute and obtuse,

respectively, figures 179 and 180.

DITRIGONAL SCALENOHEDRAL CLASS. 61

Fig. 181. Fig. 182. Fig. 183.

~ u (a:oca:a:mc] mP T

The symbols are _ | ; + ,K\hohl\, figure

183;

, K\ohhl\,

figure 181.

The principal crystallographic axis

passes through the two equal

trihedral angles, the secondary axes bisect opposite lateral edges.

These axes indicate the directions of those of trigonal and binary

symmetry, respectively.

Scalenohedrons.

Every dihexagonal bipyramid gives rise to two

congruent forms, bounded by twelve similar scalene triangles, called

scalenohedrons, of which one is

positive and the other negative,

figures 184 to 1 86. Each possesses six obtuse and six more acute

polar edges, also six zigzag lateral edges. As is the case with the

rhombohedrons, obtuse and acute scalenohedrons are possible,

depending upon the value of a : c.

Fig. 184. Fig. 185. Fig. 186,

62 HEXAGONAL SYSTEM.

a\mc\

._,

. :

The \na :pa symbols are : -fm

Pn

,

K\hikl\, figure

186; - , figure 184.

Scalenohedrons with twelve equal polar edges are crystallographically

impossible, see page 49.

The axis of trigonal symmetry passes through the two hexahedral

angles, while those of binary symmetry bisect the lateral edges.

The other holohedral forms remain unchanged by the application

of the rhombohedral hemihedrism, compare figures 178, 182, and 185.

Abbreviated Symbols of Naumann. In order to more easily

express some of the interesting relationships existing between forms

of this class, which are quite common,

Naumann

substituted for

P

and-f

Fig. 187.

the symbols of the rhombohedrons used

above, +R and 4^ mR, respectively. For

every rhombohedron there exists a series of

scalenohedrons, whose lateral edges coincide

with those of the rhombohedron, as

shown in figure 187. The inscribed rhombohedron

is known as "the rhombohedron

of the middle edges. The scalenohedrons

may, therefore, be indicated

"

in

general by mRn, mR representing the

"rhombohedron of the middle edges.

"

In

mRn, n has reference to the value of the c

axis 1} of the scalenohedron in respect to that

of the rhombohedron mR. For example,

in figure 187, the length of the c axis of the

scalenohedron is three times that of the

inscribed positive unit rhombohedron. The

symbol for this scalenohedron is, hence, according to Naumann -{-R3.

The prism of the first order OoP, also the basal pinacoid OP,

are often written QoR and OR, respectively. The symbols for the

other forms mP2, QoP2, ooPw, remain unchanged.

And not to the secondary axes, as is usually the case in the regular Naumann symbols.

DITRIGONAL SCALENOHEDRAL CLASS.

To transform the full into the abbreviated symbols and vice

versa, the following formulae are useful:

n

__^

4PI =

2 n 2

2.

mnP 2H . For example, 2R2 = -.

R Here,

=

v

K 2R2.

I 2k ti

4. mRn = K

3. *\hikl\

=

'.

(n i).

- (n

-\- i).

~\- For

2R2 = ^4131}.

instance,

The principal features of the forms of this class are given

following table:

in the

64 HEXAGONAL SYSTEM.

Combinations. Many of the more common minerals crystallize

in this class, for example, Calcite, CaCO 3

; Hematite, Fe 2

O 3

Corundum,

A1 2

;

O 3

and

; Siderite, FeCO .

3

Fig. 188. Fig. 189. Fi- 190. Fig. 191.

Figure 188. r = R, K j

101 1 \ ;

c = OR, K\OOOI}._

Calcite.

Figure 189. e = ^R, K{oii.2} ;

m

= OoR, K

\

ioTp}.

Calcite.

Figure 190. e = iR, K{oii2(; a = OoPa, K{ 1

120}. Calcite.

Figure 191. r = R, K{IOII}; /= 2R, K {o22i\. Calcite.

Fig. 192. Fig. 193. Fig. 194.

Figure 192. v = RS, KJ2I3I}; r = R, KJIOII}. Calcite.

Figure 193. r R, KJIOII}; v = R3, ^{21^1 \

._ Calcite.

Figure 194. c = OR, K{OOOI } ; m

;

=

QC-P2, K-Jii2o}. Calcite.

= OoR, K{ loiol ;

s = R\$

Fig. 195. Fig. 196. Fig. 197.

,

{na\pa\a\

I

HEXAGONAL BIPYRAMIDAL CLASS. 65

K{IOII|.

Figure 195. d = OR, KJOOOI|; r = R,

Corundum.

Figure 196. d OR, K|OOOI|; r R,

KJioiif ; n = |P2, KJ2243J; I = OoP2, K

{

1

120}.

Corundum.

Figure 197. r = R, KJIOII};

r' = R,

K\ioi4\', p = |P2,

K

1 2243}. Hematite.

Figure 198. r = R, KJIOII j; 4r = 4R,

*J404il; w = R5, S325i}; * = R3 KJ2i3if;

g-

= ooR, K{ loioj. Calcite.

Fig. 198.

6. HEXAGONAL BIPYRAMIDAL CLASS.*)

(Pyramidal Hemihedrism.)

Symmetry. The secondary and intermediate planes and the

six axes of binary symmetry are lost. The remaining

elements are

the principal plane, the hexagonal axis and the center of symmetry,

figure 203, page 66.

Hexagonal bipyramids of the third order. Figure 200 illustrates

the pyramidal method of extension and suppression of faces

on the dihexagonal bipyramid. It is obvious that this bipyramid

yields two new forms, each bounded by twelve equal isosceles triangles.

They are termed positive (figure 201) and negative*^ (figure

the third order. In form these

199) hexagonal bipyramids of

bipyramids do not differ from those of the first and second orders.

Figures 202 and 204 show the positions of these bipyramids in

respect to the secondary axes. The inner and outer light outlines

represent the horizontal cross-sections of the bipyramids of the first

and second orders, respectively, while the heavy outlines show the

cross-sections of those of the third order. These occupy an intermediate

position.

The symbols are: +

me]

,

~ '

I

4

mPn

i~

TT\/likl\

fig-

iare2Oi; , ir\ihkl\ figure 199.

I)"

Called by Dana the pyramidal group,

2) The terms right and left are sometimes used.

66 HEXAGONAL SYSTEM.

The axis of hexagonal symmetry passes through the hexahedral

angles. The position of the secondary crystallographic axes is shown

by figures 202 and 204. These do not join the tetrahedral angles

or the centers of the basal edges, but some point between them,

which is

dependent upon the value of n. Compare figures 135 to 136.

Fig. 199.

Fig. 200.

Fig. 202.

Fig. 203.

Fig. 201.

Fig. 204.

Fig. 205. Fig. 206. Fig. 207.

HEXAGONAL BIPYRAMIDAL CLASS. 67

Hexagonal prisms of the third order. From the dihexagonal

prism two congruent forms consisting of six planes, the positive

(figure 207) and negative (figure 205) hexagonal prisms of the

third order are derived. Figures 202 and 204 show these forms and

their relation to the other hexagonal prisms. Their position in

regard to the secondary axes is the same as for the bipyramids of this

order.

_,

na :

The

:pa a : ccc ooPn

symbols are: _

;H \hiko

figure 207; , Tt\ihko\ figure 205.

The axis of hexagonal symmetry extends parallel to the edges.

The other holohedral forms are unaltered by the application of

the pyramidal hemihedrism, since the suppression effects only one half

of each face. Compare figures 200, 203 and 206. They are, hence,

apparently holohedral.

The principal features of this class have been summarized in the

following table:

68 HEXAGONAL SYSTEM.

Combinations. Figure 208. m = oop ?

c =

; OP, TrjoooiS; x -- P, TrjiouJ;

5 = 2P2, irjll2l|; U = +

ir

, I j 231}. This

combination has been observed on apatite,

Fig. 208.

Ca 5Cl(P04),

. 209.

HBXAQONAL TRAPBZOHEDRAL CLASSY)

( Trapezohedral Hemihedrism. )

Symmetry.

The center and all planes

of symmetry disappear. Hence, the elements

of this class are the hexagonal axis

and six binary axes of symmetry, figure 209.

Hexagonal Trapezohedrons. From

figure 211 it is evident that by means of this

hemihedrism, the dihexagonal bipyramid

yields two correlated forms bounded by

similar trapeziums. The forms are enantiomorphous

and designated as the right

and left hexagonal trapezohedrons.

Fig. 210.

Fig. 211.

Fig. 212.

Their symbols are: r, I

f na :

_ in Pn

figure 212; l,T\kihl\ figure 210.

fia a * me]

: :

.

:

, r\hikl\

1) Trapezohedral group of Dana.

HEXAGONAL TRAPEZOHEDRAL CLASS. 69

On the right trapezohedrons the six longer basal edges are

inclined to the left of the observer and, vice versa, to the right in the

case of the left form, compare figures 212 and 210.

The axis of hexagonal symmetry joins the hexahedral angles.

The secondary crystallographic axes connect the centers of the longer

basal edges, the intermediate those of the shorter. These axes

possess binary symmetry.

Since this hemihedrism calls for the suppression of only portions

of each of the faces of the other holohedrons, no new forms can be

derived from them.

They are apparently holohedral.

The chief features of the forms of this class are given

following table:

in the

70 HEXAGONAL SYSTEM.

No crystals showing the occurrence of the hexagonal trapezohedrons

have as yet been discovered. The double salt, barium stibiotartrate

and potassium nitrate, Ba(SbO) 2 (C4H 4

O 6 ) 2 + KN O 3 ,

and the

corresponding lead salt are assigned to this class. The crystals are

apparently holohedral, the etch figures, however, reveal the lower

7. DITRIQONAL PYRAMIDAL CLASS.V

( Trigonal Hemihedrism with Hemimorphism. )

Fig. 213.

Symmetry. If the forms of the ditrigonal

bipyramidal class, page 56, become

hemimorphic, the principal plane of symmetry

and, of course, the axes of binary symmetry

also are lost. Three intermediate planes and

a polar axis of trigonal symmetry parallel to

the c axis are the only elements left. These

symmetry relations are shown in figure 213.

The forms of this class may, moreover, be considered also as

derived from those of the ditrigonal scalenohedral class, that is, from

those showing rhombohedral hemihedrism, page 60. A comparison

of figures 159 and 178 reveals the fact that when hemimorphism

becomes effective the resulting forms must in both cases be the same.

Therefore, this class is often known as the rhombohedral hemimorphic

class.

Trigonal pyramid of the first order. The trigonal bipyramid,

page 56, the result of the application of the trigonal hemihedrism to

the hexagonal bipyramid of the first order, yields upon the addition

of hemimorphism upper and lower forms, consisting of but three

faces each. Since there are two trigonal bipyramids, one positive

and the other negative,

it follows that each hexagonal bipyramid of

the first order now yields four forms. 2)

are termed trigonal pyramids.

3)

Being singly terminated, they

!) Called by Dana the rhombohedral hemimorphic class.

2) The forms are, hence, sometimes said to be the result of tetartohedrism, namely the ditrigonal

Pyramidal tetartohedrism .

3) Compare footnote on page 51. The letters u and / designate the upper and lower forms,

respectively.

u,

\

u,

DITRIGONAL PYRAMIDAL CLASS. 71

Their symbols are: f a : oo a :

I

Positive upper, +

a : mc\ m P

~u, \hohl\.

f : oo a : a

:

. m

P .

7 -

me]

Positive lower, -H /, + -/, {Ao A/}.

4 4

:

fa oca a : :

me]

Negative upper, - -

:

[a oca a me] :

Negative lower, - /,

:

mP

\u, - u, \o/i/il\.

mP

- -

/, \ohhl\.

Hexagonal pyramids of the second order. The hexagonal

bipyramid of this order remains unaffected by the trigonal hemihedrism,

page 59, but now yields an upper and lozuer form, each

consisting of six faces, termed hexagonal pyramids of the second

order.

:

:

mP2

( 2a : 2a a me^

The symbols are: \u, 1; 1

^-U {hh2hl\,

?, \hh~2lil\.

Ditrigonal pyramids. The dihexagonal bipyramid by means

of the trigonal hemihedrism yields the positive and negative ditrigonal

bipyramids, page 57. Each of these bipyramids now gives rise to

an upper and lower form, termed ditrigonal pyramids.

1}

These,

like the preceding pyramids of this class, are open forms. They

consist of six faces.

The symbols are:

Positive upper, -

Positive lower,

:

:

mPn

:

[na pa a me]

-\ u, \hik l\.

I 4 J 4

na: Pa:a:me] ^ + mPn ^

--

!) Since, as said on page 70, these forms may be considered as derived from those showing

rhombohedral hemihedrism, the terms rhombohedron- and scalenohedron-like faces are sometimes used

for the trigonal and ditrigonal pyramids, respectively, the forms being assumed to be half of the

rhombohedron and scalenohedron.

I

I---I

72 HEXAGONAL SYSTEM.

:

\na - pa :a me} mPn -- ,7-75

:

I

Negative upper, , u, \thkl\.

I 4 J 4

Negative lower,

Trigonal prisms.

^ na : :

pa a :

-

mc\ ,.,--=,

- -

/,

/, {thkl\.

I 4 J 4

mPn .

Hemimorphism does not affect, morphologically,

the trigonal prisms, the hemihedrons of the hexagonal prism

of the first order, page 56, for each face belongs alike to the upper

and lower poles.

a: aoa:a: ccc OoP

~

The symbols are : +

J

-

\nono\\

Hexagonal prism of the second order. It will be recalled that

the hexagonal prism of this order remains unchanged, geometrically,

by the trigonal hemihedrism, page 59. Hence, as in the preceding

case, each face belongs alike to the upper and lower poles, hemimorphism

also can not be effective in the production of new forms.

This prism is, therefore, still

apparently holohedral.

Its symbols are: 2a : 2a

Ditrigonal prisms.

: a :

one, ooP2, \hh2ho\.

As in the case of the trigonal prisms, page

59, these forms remain unchanged.

\

(na pa :a\ ace] ccPn

The symbols are :

+

; ,

\htko\\

QQ Pn

-f^

These, together with the trigonal prisms, are not to be distinguished

morphologically from those of the ditrigonal bipyramidal

class. They are apparently hemihedral.

Basal pinacoids. This form now evidently consists of two

types, upper and lower, of one face each.

oca : oca : oca :

f c] OP

-

/,

2

The symbols are:

--

(,/, :- u, 5oooi};

0001 .

1 1

In all the above forms the crystallographic axes are located as

in the ditrigonal bipyramidal class.

DITRIGONAL PYRAMIDAL CLASS. 73

The following table shows the principal features of the forms of

this class:

Combinations. The mineral tourmaline furnishes excellent

combinations of the above forms.

74 HEXAGONAL SYSTEM.

Fig. 215.

In the accompanying figures

P -

214 and 215, P = 4- u, {

ion } ;

4

P __ 2 P

P = +

-

/, Join | ;

o = -- w,

4 4

OP

50221 i; c - I, {oooij; n

OOP

f. .

H20

t = + u, 2131;

= / lOIIOj

4 2

As indicated on page 70, these forms may be assumed as

derived from those of the ditrigonal scalenohedral class, i. e., showing

rhombohedral hemihedrism, and, hence, are often designated as

follows :

= ooP2; / --;

ooR

o = 2Ru.

=

; c= I

Fig. 216.

8. HEXAGONAL PYRAMIDAL CLASS.

(Pyramidal Hemihedrism with Hemimorphism.)

Symmetry.

This class possesses but one

element of symmetry, namely, a polar axis of

hexagonal symmetry, as shown in figure 216.

This is obvious, for when the forms of the hexagonal

bipyramidal class, page 65, become

hemimorphic, the principal plane and center

of symmetry are of necessity

lost. Forms of

exactly the same character are, moreover, to

be derived by applying hemimorphism to those

of the hexagonal trapezohedral class. Compare figures 203 and 209.

Forms. The bipyramids of the first, second and third orders of

the hexagonal bipyramidal class 1} now consist of upper

and lower

1) If, however, hemimorphism be applied to the hexagonal trapezohedral forms, the hexagonal

trapezohedrons and dihexagonal prism would yield forms corresponding precisely to the pyramids and

prisms of the third order. The other forms being apparently holohedral in both classes would, of

course, be affected alike by the introduction of hemimorphism.

HEXAGONAL PYRAMIDAL CLASS. 75

of an

pyramids. The prisms, on the other hand, remain unaffected morphologically.

The basal pinacoid, of course, is now composed

upper and lower form.

As in the preceding class, these are now open forms. Their

position in respect to the crystallographic axes is the same as in the

hexagonal bipyramidal class, page 65.

The principal features are given in the following table:

Combinations. By means of etch figures crystals of a number of

compounds have been referred to this class. Among the minerals,

76 HEXAGONAL SYSTEM.

nepheline, Na 8

Al 8

Si 9

O 34 ,

is to be mentioned. Figure 217

shows a crystal of strontium antimonyltartrate, Sr (SbO) 2

p

= ~u, {ion

-/, J202IL

HEXAGONAL TETARTOHEDRISMS.

The tetartohedral forms may

be assumed as derived

from the holohedral by applying simultaneously two types

Fig. 217. of hernihedrism, page 55. Thus, by combining the trigonal

and pyramidal hemihedrisms, the trig-onal tetartohedrism

results, figure 218. A second type, known as the trapezohcdral

tetartohedrism, is the result of the combination of the

Fig. 218. Fig. 219. Fig. 220.

rhombohedral and trapezohedral hemihedrism, figure 219. The

simultaneous application of the rhombohedral and pyramidal hemihedrisms

gives rise to the rhombohedral tetartohedrism, figure 220.

These three are the only types possible, for other combinations

of the four methods of hemihedrisms do not

satisfy the conditions of tetartohedrism.

9. TRIGONAL BIPYRAMIDAL CLASS.

( Trigonal Tetartohedrism. )

This class possesses two ele-

Symmetry,

ments of symmetry, namely, a principal plane

Fig. 221 and an axis of trigonal symmetry, figure 221.

TRIGONAL BIPYRAMIDAL CLASS. 77

Trigonal b i

p y r a-

mids and prisms of the

first order. As can be

222 and 223, the hexagonal

bipyramids and

prism of the first order now

yield trigonal bipyramids

and prisms, respectively.

These forms do not differ

from

morphologically

those of the ditrigonal bipyramidal class, compare figures 160 to 168.

The symbols for the trigonal bipyramids of the first order are:

a : oca : a : .

me]

^~ + ,

-J,

a :

ooa

:

a :

me]

Fig. 222. Fig. 223.

mP

\hohl\\ and

mP

,

J,

Those for the corresponding trigonal prisms being:

a : oca : a : ooc

-

, {ohhl\.

ocP

+ \hoho\\ and

a :

cca

:

a

:

-, \ohho\.

Trigonal bipyramids and prisms of the second order.

forms are obtained from the hexagonal bipyramid and prism

These

of the

Fig. 224. Fig. 225. Fig. 226.

Fig. 227. Fig. 228. Fig. 229.

I

78 HEXAGONAL SYSTEM.

second order as can be seen from figures 224 to 229. The position

of these forms as well as those of the other two orders in respect to

the crystallographic axes is shown in figure 237.

The symbols for the trigonal bipyramids of the second order:

( 2a : 2a

I

: 2a :

a

:

me ?;z P 2

me

-

,

^-, 2 hhhl\, figure 224.

J

{h h 2 hl\, figure 226; and

Those of the corresponding trigonal prisms:

2a : 2a : a : ooc] ocP2

, \h1i2ho}, figure 229, and

\2a : 2a : a : ooc] Gc?2

-

,

2

( J

2

, | 2 h h h o \

,

figure 227.

Trigonal bipyramids and prisms of the third order. The

dihexagonal bipyramid now furnishes four new forms, termed trigonal

bipyramids of the third order, while the dihexagonal prism

yields the corresponding prisms. Figures 230 to 235 show the

derivation of two forms of the bipyramid and prism. Figures 236

and 237, however, show the position of these forms in respect to the

crystallographic axes as also to the forms of

the other orders.

Fig. 230. Fig. 231. Fig. 232.

Fig. 233. Fig. 234. Fig. 235.

TRIGONAL BIPYRAMIDAL CLASS. 79

The symbols of the bipyramids are:

Positive right,

:

{ na :

pa

+ r [~ ~2~

a : me

Positive left,

; ^na-.pa-.a-.mc^ +

.

.

{hikl}, figure 232.

.

,

\kihl\, figure 230.

Negative right,

I

2

_

J 4

Negative left,

{ na :

pa

:

a : me

-I- -; \khil\.

Those of the prisms are:

[ na : pa

:

a : Gc

2

; \hiko\i figure 235.

; \kiho\, figure 233.

na:pa:a:aoc] QcPw .,-r

( i

r\-

I; r

;

-j- ~^

jiA^o}.

Fig. 236. Fig. 237.

The basal pinacoid, as is obvious from figures 223,

remains unaltered.

^28 and

80 HEXAGONAL SYSTEM.

The following table summarizes the principal features of each

form.

No representative of this class has yet been discovered.

TRIGONAL TRAPEZOHEDRAL CLASS. 81

10. TRIGONAL TRAPEZOHEDRAL CLASS.*)

( Trapezohedral Tetartohedrism. )

A principal axis of trigonal

Symmetry.

symmetry and three polar axes of binary

symmetry are the only elements in this

class, figure 238.

Rhombohedrons of the first order.

From the hexagonal bipyramid of the first

order, two rhombohedrons of the same

order result as can be seen from figure 239.

These forms are identical, morphologically,

with those of the ditrigonal scalenohedral

class, page 60.

Their symbols are: Hr , {a:Cioa:a:

'

me

+ mR, \ho7il\\ mR, \oh7il\. 2}

Trigonal bipyramids of the second

order. The hexagonal bipyramids of the

second order, figure 240, yield two trigonal

bipyramids of this order. They are identical,

geometrically, with those of the trigonal

bipyramidal class, page 77. 3

The symbols are:

I\ 2a\ ia \a\mc

Fig. 238.

Fig. 239.

Trigonal Trapezohedrons.

The dihexagonal

bipyramids yield four new forms,

each bounded by six faces, which in the

ideal development are equal trapeziums.

Figure 242 shows the application of the

trapezohedral tetartohedrism so as to give

Fig. 240.

rise to the positive right trigonal trapezohedron, figure 243. Figure

241 shows the positive left form. These are enantiomorphous.

1) The trapezohedral group of Dana .

2 )

Sometimes the two Greek letters K T are placed before the Miller indices. See footnote on

page 40. 3) Sometimes designated as right and left.

^mPn

82 HEXAGONAL SYSTEM.

The trigonal trapezohedrons may also be conceived as derived

from the scalenohedron by the subsequent application of hemihedrism.

This is shown by figure 245, a negative scalenohedron, which

now yields the negative right (figure 246) and negative left

244) trigonal trapezohedrons, respectively.

(figure

Fig. 244. Fig. 245. Fig. 246.

The symbols may be written as follows:

i) Positive right,

na\pa\a\mc\

,

-j-

j

,

.

-h r -

,

r l

\hikl\> figure 243-

TRIGONAL TRAPEZOHEDRAL CLASS. 83

)

Positive left,

f na : :

pa a : .

me]

-h / H- / -

,

L 4 J 4

. mPn

3) Negative right,

na : :

pa a :

me]

r

4 4

mPn

*

\k i h l\ , figure 241.

i h k /}, figure 246.

4) Negative left,

na : :

pa a :

me] _

mPn

4 J' 4

'

k h i /}, figure 244.

Forms i and 2, 3 and 4 are among themselves enantimorphous,

while i and 3, 2 and 4 are congruent.

The polar axes of binary symmetry bisect the zigzag edges.

Trigonal prisms of the second order.

Figure 247 shows that the hexagonal prism

of this order yields two trigonal prisms.

These are similar to those of the trigonal

bipyramidal class, page 77.

The symbols are :

+

-, \hh2ho\\

OCP2

2 h h h o

Ditrigonal Prisms. The dihexagonal Fig 247.

prism now gives rise to two ditrigonal prisms

as shown in figures 248, 249 and 250. These are similar, morphologically,

to those of the ditrigonal bipyramidal class, page 59, but

differ from them in respect to the position of the crystallographic axes.

A comparison of figures 251 with 172 and 174 shows the difference.

Fig. 248. Fig. 249. Fig. 250.

\na

84 HEXAGONAL SYSTEM.

,

,~, : -ha : a :Ooc

The symbols are : Hr -

, \hiko\t

1 ; -ffigure

250; -

-, \ki7io\, figure

Fig. 251. Fig. 252. The other forms,

hexagonal prism

of the first order and

the basal pinacoid,

remain unchanged,

figure 252.

The important

features of this class

given in the following

*) Often designated as right and left forms.

UNIVERSITY 1

C4L!?

TRIGONAL RHOMBOHEDRAL CLASS. 85

Combinations. Quartz, SiO 2 , and Cinnabar, HgS, furnish

excellent examples of minerals crystallizing in this class.

Fig. 253. Fig. 254. Fig. 255.

Figures 253 and 254. a oo R

j

ioio( ; r = + R

{

= R{oiu}; \$ (figure 254)

=

+ -{ Il2 i}, (figure253)

21 fi}; * (figure 254) = + r

Figure 255. r =

- [

;

w

101 1 j ;

2P2

JS^il, (figure 253) + /-

4 4

= OoR{ioio}; r = -f R{ ion | ;

-IP4

g- = iR|oii2(; n' =

2R|o22ii; and x = + / ^-^ 18355. J

Cinnabar.

//. TRIGONAL RHOMBOHEDRAL CLASS. 1 )

Symmetry.

(

Rhombohedral Tetartohedrism. )

This

class possesses a principal

axis of trigonal

symmetry. A center

,

of symmetry is also

present, figure 256.

Rhombohed r o n s

of the first order. The

Fig. 256.

hexagonal bipyramid

of the first order, figure 257, now yields two

Fig. 257.

rhombohedrons which are identical, geometric-

The tri rhombohedralgroup oi Dana.

, \2a

I

HEXAGONAL SYSTEM.

ally, with those of the ditrigonal scalenohedral class, page 60,

figures 179 and 181.

The symbols are:

f a :

00 a : a

:

mc\

\ mR{o/i/il\.

Rhombohedrons of the second order. Figure 259 shows the

application of rhombohedral tetartohedrism on the hexagonal bipyramid

of the second order. This form now yields the rhombohedrons

of the second order.

Fig. 258.

Fig. 259. Fig. 260.

The symbols are:

2a : : a

:

me

+ - \hh2hl\ figure 260;

2 h h h 1 l\ figure 258.

Rhombohedrons of the third order. From the dihexagonal

bipyramid four rhombohedrons of the third order result. Two of

Fig. 261. Fig. 262. Fig. 263.

TRIGONAL RHOMBOHEDRAL CLASS. 87

these are shown in figures 261, 262 and 263. The position of these

rhombohedrons with respect to the crystallographic axes is shown by

figures 236 and 237, which also indicate the relation existing between

the rhombohedrons of the three orders.

The symbols are:

Positive right,

na :

pa a

:

4

:

me}

mPn

(

r-

,

4

, . r ,) ^

\hikl\, figure 263.

Positive left,

f na :

pa

:

'

a

4

Negative right,

f na : :

pa

r

~~4~~

: me

a : me

,wPw

4

mPn

r

\ki hl\, figure 261.

\ihkl\.

\k~hil\.

Negative left,

w :

C ^>

: : w

Hexagonal prisms of the third order.

Figure 264 shows that the dihexagonal prism

now yields two hexagonal prisms of the third

order. Compare figures 205 and 207.

The symbols are:

oo P^

\na \pa :a: ccPn r

\hiko\-,

\kiho\.

Fig. 264.

Other

forms.

The remaining holohedrons

are unchanged

by this tetartohedrism,

see figures 265 and

266.

Fig. 265. Fig. 266.

88 HEXAGONAL SYSTEM.

The principal features may

be tabulated as follows:

Three equal edges.

jioiij;

TRIGONAL PYRAMIDAL CLASS. 89

Combinations. Dolomite, CaMg(CO 3 ) 2 , and dioptase, J^CuSiO^

crystallize in this class.

Figure 267. m = OcP2, j 1

120} ;

r = 2R, 5

022 1 j ;

5 = / * ,

{18. 17. 1.8}, dioptase.

r = R,

.

Figure 268. m = 4R, {4041 } ;

VP 2

?z =

>

5i6.8-8.3j 1 >; *:

= OR, {oooi}, dolomite.

Fig. 268.

12. TRIGONAL PYRAMIDAL CLASS.

[Ogdohedrism.

Trigonal Tetartohedrism with Hemimorphism.)

"]

Symmetry. The only element of symmetry is a polar

trigonal symmetry parallel to the c axis, figure 269.

axis of

^Mp

Forms. When hemimorphism becomes effective on forms of

the trigonal bipyramidal class, page 76, it is evident the various

bipyramids and the basal pinacoid give rise to upper and lower forms.

The prisms, however, remain unchanged since they belong alike to

the upper and lower poles.

The principal features of these forms are given in the following

table:

Rhombohedron of the second order.

90 HEXAGONAL SYSTEM.

TRIGONAL PYRAMIDAL CLASS.

91

Combination. Figure 270. r= +

= - - w, J022I}; ^=/,

joooij; /=

periodate, NaIO 4

+ 3H 2

O.

P

_

2134}. Sodium

Fig. 270.

TETRAGONAL SYSTEMS

Crystallographic Axes. The tetragonal system includes all

forms which can be referred to three perpendicular axes, two of which

are equal and lie in a horizontal plane.

These are termed the secondary or lateral

axes and are designated as the a axes. Perpendicular

to the plane of the lateral axes is

the -principals? c axis, which may be longer

or shorter than the a axes. The axes,

which bisect the angles between the a axes,

are the intermediate axes. They are

designated as the b axes in figure 271.

Crystals of this system are held so that

the c axis is vertical and one of the a axes

-c

is directed towards the observer.

Fig. 271.

Since the lengths of the a and c axes

differ, it is

necessary to know the ratio existing between these axes,

that is, the axial ratio, as was the case in the hexagonal system.

Compare pages 7 and 43.

Classes of Symmetry.

symmetry, as follows: This system embraces seven classes of

1 .

Ditetragonal bipyramidal class (Holohedrism.)

7. Tetragonal bisphenoidal class ( Tetartohedrism).

{ Holohedrism and}

2. Ditetragonal pyramidal class

\hemimorphism. J

3. Tetragonal scalenohedral class 1

4. Tetragonal bipyramidal class .

\ (Hemihedrism)

5. Tetragonal trapezohedral class j

[Hemihedrism and\

6. Tetragonal pyramidal class

\hemimorphism. J



Also termed quadratic or pyramidal systei

DITETRAGONAL BIPYRAMIDAL CLASS. 93

Classes i , 3 and 4 are the most important,

of class 7 has yet been observed.

No representative

DITETRAQONAL BIPYRAMIDAL CLASS. 1 )

(

Holohedrism. )

Symmetry, a) Planes* In this class

there are five planes of symmetry. The

plane parallel to the plane of the secondary

and intermediate axes is termed the

principal plane. The vertical planes including

the c and one of the a axes are called

the secondary planes, while those which

include one of the b axes are termed the

intermediate planes, figure 272.

The principal and secondary planes

divide space into eight equal parts, termed

octants. The five planes, figure 272,

divide it into sixteen equal sections. The

five

planes may be designated as follows:

i

Principal -h 2 Secondary + 2 Intermediate

= 5

Planes.

b) Axes. Parallel to the c axis, there

is an axis of tetrag-onal symmetry. The

axes parallel to the secondary and intermediate

axes possess binary symmetry,

figure 273. These may be written: i|

-}-2+20:=5 axes.

c) Center. A center of symmetry is

also present in this class. These elements

of symmetry are shown in figure 274, which

represents the projection of the most complex

form upon the principal plane of symmetry.

Fig. 273.

Flg * 2 ' 4 *

Tetragonal bipyramid of the first order. This form is analogous

to the octahedron of the cubic system, page 19. But since

1) The normalgroup of Dana.

94 TETRAGONAL SYSTEM.

the c axis differs from the secondary axes, the

ratio must be written (a

: a :

c\ which would

indicate the cutting of all three axes at unit

distances, 1 )

figure 275. But since the intercept

along the c axis may be longer or shorter

than the unit length, the general ratio would

: a :

me), where m is some value

between zero and infinity. Like the octahedron,

this form, the tetragonal bipyramid,^

is bounded by eight faces which enclose space.

Fig 275. The faces are equal isosceles triangles when

the development is

The Naumann and Miller symbols are:

ideal.

P, | in}; or raP, \hhl\.

The principal crystallographic axis passes through the two tetrahedral

angles of the same size, the secondary axes through the other

four equal tetrahedral angles, while the intermediate axes bisect the

horizontal edges.

Tetragonal Mpyramid of the second

order. The faces of this form cut the c

and one of the a axes, but extend parallel

to the other. The parametral ra,tio is,

therefore, a : O0 : me. This requires

eight faces to enclose space and the form

is the bipyramid of the second order,

figure 276. The symbols according to

Naumann and Miller are: raPoc, \ohl\.

In form this bipyramid does not

Fig. 276. differ from the preceding, but they can

be readily distinguished on account of

their position in respect to the secondary axes. In this form, the

secondary axes bisect the horizontal edges and the intermediate

axes pass through the four equal tetrahedral angles. This is the

1) Indicating a unit form, compare page 7.

2) The more the ratio a : c approaches 1 : 1, the more does this form simulate the octahedron.

This tendency of forms to simulate those of a higher grade of symmetry is spoken of as pseudo symmetry.

DITETRAGONAL BIPYRAMIDAL CLASS. 95

opposite of what was noted with the bipyramid of the first order,

compare figures 275 and 276. Hence, the bipyramid of the first

order is always held so that an edge is directed toward the observer,

whereas the bipyramid of the second order presents a face. In both

bipyramids the principal axis passes through the two equal tetrahedral

angles.

Ditetragonal bipyramid. The faces of

this bipyramid cut the two secondary

axes at

different distances, whereas the intercept along

the c axis may be unity or me. Sixteen such

faces are possible and, hence, the term ditetrag-onal

bipyramid is used, figure 277. 1}

The symbols are:

(a\na:mc\ mPn, \hkl\.

Since the polar edges

2)

are alternately

dissimilar it follows that the faces are equal,

Fig. 277.

similar scalene triangles. The ditetragonal

bipyramid possessing equal polar edges is crystallographically an

impossible form, for then the ratio a : na : me would necessitate a

value for n equal to the tangent of 67 30', namely, the irrational

3)

value .

2.4i42 +

From the above it follows that when n is less than 2.41424- the

ditetragonal bipyramid simulates the tetragonal bipyramid of

order, and finally when it

equals I, it

passes

over into that form. On the other hand, if n

is greater than 2.4142+ it approaches more

the bipyramid of the second order, and when

it is

equal to infinity passes

over into that

form. Hence, n > I < oo. Figure 278 illustrates

this clearly. It is also to be noted,

that when n is less than 2.4142-!- the secondary

axes pass through the more acute angles,

whereas, when n is greater than 2.4142 +

Fig. 278.

the first

they join the more obtuse. In figure 278, outline I

represents the

cross-section of the tetragonal bipyramid of the first order, 2 that

*) Compare figure 24, page 10.

3 ) Compare footnote, page 48.

96 TETRAGONAL SYSTEM.

of the second order, and 3, 4 and 5 ditetragonal bipyramids where n

equals f , 3, and 6, respectively.

Tetragonal prism of the first order.

If the value of the intercept along the c

1_

axis in the tetragonal bipyramid of this

order becomes infinity,

faces of the bipyramid

the number of the

is reduced to four

giving rise to the tetragonal prism of

the first order, figure 279. This is an

open form and possesses the following

symbols:

(a : a

: aoc), ooP, | noj.

The secondary axes join opposite

edges, hence, an edge

is directed toward

the observer.

JL-.

Fig. 280.

Fig. 281. Tetragonal

order. The same

between this form

bipyramid as was

form.

The symbols

(a: oca: ooc),

This is also

ing of four faces,

ondary axes join

site faces. Hence,

toward the observer.

Ditetragonal

this form consists

ing the following

a:na:Ooc,

What was said

ing the polar angles secondary axes

Figure 281 represents

prism.

prism

relationship

and are:

ooPoo,

an open

figure a

prism.

of eight

symbols:

OoPw,

on page

and

applies

of

its

corresponding

form

280.

face

As

faces

\hko\.

the

a

the

preceding

jioo}.

The is

is

94 concern-

position

here

ditetragonal

second

exists

consist-

sec-

oppo-

directed

obvious,

possess-

of

also.

1

DITETRAGONAL BIPYRAMIDAL CLASS. 97

Basal Pinacoid. This form is similar to that of the hexagonal

system, page 51. It is parallel to the secondary axes but cuts the

c axis. The symbols may be written :

(ooa

:

oca :

c], OP, jooif.

This form consists of but two faces. They are shown in combination

with the three prisms in figures 279, 280, and 281.

These are the seven simple forms possible in the tetragonal

system. The following table shows the chief characteristics of each.

TETRAGONAL SYSTEM.

Relationship of forms. This is clearly expressed by the following

diagram. Compare pages 23 and 52.

oca : oca : c

a :

oca

:

me

a :

7ia : me

a :

oca

:

occ

a : na :

Oc c a :a : occ

Combinations. Some of the more common combinations are

illustrated by the following figures:

Fig. 282. Fig. 284. Fig. 285.

Figures 282 to 286. m ^ooPjuoj, p Pjin}, a =

OoPocJioo}, u = 3PS33M. v=~- 2P|22i|, and x - 3P3J3ii}.

These combinations are to be observed on zircon, ZrSiO 4

.

Fig. 286 Fig. 288. Fig. 289,

DITETRAGONAL PYRAMIDAL CLASS.

Figure 287. m< = OoP uoJ, a = OoPoo

JioiJ, and 5 = Pjiiij. Cassiterite, Sn 2

O 4

.

IOO

99

e =

Figures 288 and 289. p = P\m 2 =

,

c = OPjooij,

a = ooP oo j

|P|ii3}, i;=|PJii7}, w=OoP{uo}, a = ocPoojioo}, looi and

e = P oo |

101 \.

These combinations occur on Anatase, TiO 2

.

2. DITBTRAQONAL PYRAMIDAL CLASS. 1 )

(Holohedristn

with Hemimorphism.}

Symmetry. Since hemimorphism

is effective on forms of this

class, the principal plane and the four axes of binary symmetry disappear.

The remaining elements are, therefore, two secondary and

two intermediate planes and a polar axis of tetragonal symmetry,

figure 290.

Fig. 290.

Forms. The forms of this class are analogous to those of the

dihexagbnal pyramidal class, page 53, and the ditetragonal bipyramids

and tetragonal bipyramids of the first and second orders as well

as the basal pinacoid are now to be considered as divided into upper

and lower forms. For example, the ditetragonal bipyramid now

yields an upper and a lower ditetragonal pyramid, each consisting

of eight faces. The three prisms, however, remain unaltered; they

are apparently holohedral.

*) The hemimorphic group of Dana.

100 TETRAGONAL SYSTEM.

The principal features are summarized in the following table:

DITETRAGONAL PYRAMIDAL CLASS. 101

r

ip

Combinations. Figure 291. x = ^

u<

|n 3 ;

w = -

/,

Silver fluoride, AgF.H O. 2

Figure 292. a = OoP 00 100

Ill

^ r

< )

OP

c = u> }ooif w ;

X

7

= -

/, 1 1 1

Fig. 291.

Observed on penta-erythrite,

C 5

H 12

O .

4

TETRAGONAL HBMIHEDRISMS.

In this system three types of hemihedrisms

are possible, figures 293, 294 and

Fig. 292.

295.

a) Sphenoidal hemihedrism. The principal an^tw -secondary

planes divide space into octants. All faces in alternate octants

are suppressed,

the others expanded, figure 293.'-,' >'

Fig. 293. Fig. 294. Fig. 295.

b) Pyramidal Hemihedrism. The two secondary and the

two intermediate planes of symmetry divide space into eight equal

sections, figure 272. All faces lying wholly within alternate sections

are extended, the others suppressed, figure 294.

c) Trapezohedral hemihedrism. By means of the five planes

of symmetry sixteen equal sections result. In this type of hemihedrism

all faces lying wholly within such sections are alternately extended

and suppressed, figure 295.

The pyramidal and sphenoidal types of hemihedrism are the most

important.

102 TETRAGONAL SYSTEM.

3. TETRAGONAL SCALENOHEDRAL CLASS. 1 )

(Sphenoidal Hemihedrism.}

Symmetry. In this class the elements

of symmetry consist of two intermediate

planes of symmetry, two axes of binary

symmetry parallel to the secondary crystallographic

axes, and one binary axis parallel

to the principal or c axis, figure 296. The

sphenoidal hemihedrism is analogous to the

tetrahedral and rhombohedral hemihedrisms

of the cubic and hexagonal systems, respectively;

see pages

26 and 60.

Fig. 296.

Tetragonal bisphenoids. Figure 298 shows the application of

the sphenoidal hemihedrism to the bipyramid of the first order. It

is obvious from this figure that the bipyramid of the first order now

yields! two i>ew correlated forms, each bounded by four faces.

When

On

the development is ideal, these faces are equal isosceles triangles.

account of the resulting forms resembling a wedge, they are termed the

-positive and negative tetragonal bisphenoids of the first order.

Fig. 297.

Fig. 298. Fig. 299.

The symbols are :

f# : a : me

TETRAGONAL SCALENOHEDRAL CLASS. 103

The secondary crystallographic axes bisect the four edges of

equal length, while the principal axis passes through the centers of

the other two.

Tetragonal scalenohedrons.

It is readily to be seen from figure

301, that the ditetragonal bipyramid also yields two new correlated

forms. These consist of eight similar scalene triangles, and are

termed the positive and negative tetragonal scalenohedrons.

Fig. 300. Fig. 301. Fig. 302.

The symbols are:

a : na : mc\

mP n

.

;+ mPn

\hkl\ figure 300.

figure 302;

The principal axis joins the tetrahedral angles, which possess

two pairs of equal edges. The secondary axes bisect the four zigzag

edges.

The sphenoids and scalenohedrons are congruent and, hence,

the positive and negative may be made to coincide by means of a

revolution through 90

The other tetragonal forms are apparently holohedral

of figures 296, 298, and 301 will show.

as a study

The characteristics of the forms of the tetragonal scalenohedral

class may be tabulated as follows:

104 TETRAGONAL SYSTEM.

Combinations. Figure 303, m = ooP, {noj; o =

-\

,

1 1 1 1 ;

and c = OP, jooi \

.

Urea, CH 4

N 2

O.

Fig. 303. Fig. 304. Fig. 305.

Figures 304 to 307. p =

TETRAGONAL BIPYRAMIDAL CLASS.

105

-, in; r = -, in \-

e= Poo, {ioij; z = 2Poc,

|20i}; c = OP, jooi j; m

OOP, \l\Q\\t = ,

2P

22

Fig. 306.

Fig. 307.

u = P2, 5212}. These combinations

occur on chalcopyrite, CuFeS 2

.

4. TETRAGONAL BIPYRAMIDAL CLASS. 1 )

(Pyramidal Hemihedrism. )

Symmetry. The elements of this class are one principal plane,

a center, and an axis of tetragonal symmetry, as shown in figure 312.

Tetragonal bipyramids of the third order.

From figure 309 it

is obvious that by means of the pyramidal hemihedrism, the dihexagonal

bipyramid yields two new forms, each bounded by eight equal

isosceles triangles, figures 308 and 310, termed the tetragonal bipyramids

of the third order.

The symbols are:

(a : na

2

mPn

:

mc\

2

I, Tr\hkl\, figure 308.

310;

In form these bipyramids do not differ from those of the first and

second orders. Figures 3 1 1 and 3 1 3 show the positions occupied by

the bipyramids of the three orders and it is obvious that the position

of the forms of the third order is intermediate between that of the

other two.

Tetragonal prisms of the third order. In an analogous manner

the ditetragonal prism, figure 31 5, yields two correlated prisms of the

third order, each consisting of four faces. The position of these

prisms in respect to the crystallographic axes is illustrated by figures

311 and 313.

1 ) Dana's pyramidal group.

,

a

106 TETRAGONAL SYSTEM.

Fig. 314.

Fig. 315.

The symbols are:

: na

:

ccc

1

[acPn j-J,

'JAM. figure 316.

ko\, figure 314.

TETRAGONAL BIPYRAMIDAL CLASS. 107

Being open forms, they

are shown in combination with the basal

pinacoid.

Other forms.

The other holohedrons, bipyramids and prisms of

the first and second orders as also the basal pinacoid, remain unaltered

by this type of hemihedrism because their faces do not lie

wholly within the sections formed by the secondary and intermediate

planes of symmetry, compare figures 309, 312, and 315. They are,

hence, only apparently holohedral.

The chief features of the forms of the tetragonal bipyramidal

class are given in the following table:

108

TETRAGONAL SYSTEM.

Combination. Figure 317. e Poo, TT|

101 \ ;

-

I,

7^1315

This combination has been

observed on the mineral scheelite, CaWO 4

.

Fig. 317.

5. TETRAGONAL TRAPEZOHEDRAL CLASS. 1 )

( Trapezohedral hemihedrism. )

Symmetry. This class possesses a

principal axis of tetragonal symmetry and

four axes of binary symmetry. Figure 3 1 8

shows these elements as well as the application

of the trapezohedral hemihedrism.

Tetragonal trapezohedrons. The only

holohedron which can be affected by trap-

Fig. 318. ezohedral hemihedrism, page 101, is the

ditetragonal bipyramid, figure 320. This

bipyramid yields two new correlated forms, bounded by eight faces,

which are similar trapeziums, figures 321 and 319. Being enantiomorphous,

they are termed the right and left tetragonal trapezohedrons.

Fig. 319. Fig. 320. Fig. 321.

Dana rails this the traprzohcdtal group.

TETRAGONAL TRAPEZOHEDRAL CLASS. 109

The symbols are:

_ fa : na : , . _

.

7)

, r\hkl\, figure 321;

, r\hki\

t

figure 319.

Alt other forms are apparently holohedral because their faces do

not lie

wholly within each of the sixteen sections resulting from the

intersection of the five planes of symmetry.

The chief features of the forms of this class are given below:

Thus far, the tetragonal trapezohedron has not been observed

on either minerals or artificial salts. There are, however, a number

of compounds like sulphate of strychnine, (C21H 22

N 2

O 2 ) 2

H 2

SO 4 H-6H 2 O,

and sulphate of nickel, NiSO 4 +6H 2 O, which have been referred to

this class of symmetry by means of etch figures.

110 TETRAGONAL SYSTEM.

6. TETRAGONAL PYRAMIDAL CLASS. 1 )

( Pyramidal Hemihedrism with Hemimorphism. )

Symmetry. If the forms of the tetragonal

bipyramidal class, page 1 50, become

hemimorphic, the principal plane and center

of symmetry disappear. Hence, the only element

of symmetry of this class is a polar axis

of tetragonal symmetry which is parallel to

the c axis, figure 322.

Fig. 322.

Forms. The bipyramids of the tetragonal

bipyramidal class now yield upper and /oz^r pyramids. The basal

pinacoid

is also divided into two forms. The prisms remain unaltered.

Since the ditetragonal bipyramid

is now divided into four pyramids,

this class is sometimes considered a tetartohedral class.

The chief features of the forms are given in the following table:

The pyramidal-hemimorphic group of Dana.

TETRAGONAL BISPHENOIDAL CLASS.

Ill

Combination. The mineral wulfenite,

PbMoO 4

, crystallizes in this class, figure 323.

P

o = - P

~-

in o'

-

/,

; p

=

7. TETRAGONAL BISPHENOIDAL CLASSY

( Tetartohedrism. )

Symmetry. The only element of symmetry

remaining

in this class is an axis of

binary symmetry parallel to the c axis, figure

324-

Tetartohedrism. The forms of this class

may be conceived as derived from the holohedrons

by the simultaneous occurrence of

either the sphenoidal and trapezohedral, or

the sphenoidal and pyramidal hemihedrisms;

compare figures 293, 294, and 295. The

simultaneous occurrence, however, of the

pyramidal and trapezohedral hemihedrisms

give rise to the forms as described in the preceding

class.

Hi sphenoids of the first order. Figure

325 shows that the bipyramid of the first order

now yields two bisphenoids of the same order.

Compare figure 298.

The symbols are:

Fig. 325.

Bisphenoids of the second order.

The bipyramid of the second

order, figure 327, gives rise to the positive and negative bisphenoids

Dana terms this the tetartohedral group.

,

(

112 TETRAGONAL SYSTEM.

of the second order. These bisphenoids bear the same relation to

those of the first order as do the corresponding bipyramids.

Fig. 326.

Fig 327. Fig. 328.

The symbols are:

a : oca : mc\ mPoo .

figure 328;

j\hol\,

mPoo

Fig. 329. Fig. 330. Fig. 331.

Fig. 332. Fig. 333. Fig. 334.

TETRAGONAL BISPHENOIDAL CLASS. 113

.Bisphenoids of the third order. In a like manner, as is obvious,

the ditetragonal bipyramid, figure 330, yields four bisphenoids of

the third order. Figure 333 shows that these forms may also result

when hemihedrism is

applied to the tetragonal scalenohedron.

The symbols are:

mPn .

[a na me] : : _

Positive right, + r\ "+*" \khl\^ figure 321.

Positive left, -f /

Negative right,

Negative left, /

r

a : na : me

a : na : me

fa : na : me

, +/

\hkl\, figure 329.

4

mPn

, \khl\, figure 334.

/- -,\hkl\, figure 332.

The same relationship exists between the bisphenoids of the

three orders which was noted with the corresponding prisms, page

105.

In bisphenoids of

the first

order the secondary axes bisect

the zigzag edges. They join

the centers of opposite faces

in forms of the second order,

while in those of the third order

they occupy

position.

an intermediate

Fig. 335.

Prisms of the third order. Figure 335 shows that the ditetragonal

prism now yields two prisms of the third order, compare

figures 314 and 316.

The symbols are:

( a: na :

OoPn .

doe]

'

-{ 2 j

The other forms, prisms of the first and second orders and the

basal pinacoid, remain unchanged.

114 TETRAGONAL SYSTEM.

The principal features may

be tabulated as follows:

No representatives of this class of symmetry have yet been

observed,

ORTHORHOMBIC SYSTEMS

Crystallographic Axes. This system includes all forms which

can be referred to three unequal and perpendicular axes, figure 336.

One axis is held vertically, which is, as

heretofore, the c axis. Another is directed

^

toward the observer and is the a axis, sometimes

also called the brachydiagonal.

The third axis extends from right to left

and is the b axis or macrodiag'onal.

There is no principal axis in this system,

hence -C

any axis may be chosen as the vertical Fig. 336.

or c axis. On this account one and the

same crystal may be held in different positions by various

observers, which has in some instances led to considerable

confusion, for, as is obvious, the nomenclature of the various

forms cannot then remain constant. In this system the axial

ratio consists of two unknown values, viz: a\b : c = .8130:

1 :

I -937 compare page 7.

Classes of Symmetry. The orthorhombic system comprises

three classes of symmetry,

as follows:

i. Orthorhombic bipyramidal class (Holohedrism.)

Holohedrism and 1

2. Orthorhombic pyramidal class , . ...

[ hemimorphism.

3. Orthorhombic bisphenoidal class (Hemihedrism.)

Numerous representatives of all these classes have been observed

among minerals and artificial salts. The first class is, however, the

most important.

/. ORTHORHOMBIC BIPYRAMIDAL CLASS.*)

~

(Holohedrism.}

Symmetry, a) Planes. There are three planes of symmetry.

These are perpendicular to each other and their intersection gives rise

!) Sometimes termed the trimetric, rhombic, or prismatic system.

2) The normalgroup ol Dana.

116 ORTHORHOMBIC SYSTEM.

to the crystallographic axes, figure 337.

Inasmuch as these planes are all dissimilar,

they may be written:

1 + + 1=3 1 planes.

b) Axes. Three axes of binary symmetry

are to be observed, figure 337. They

Fig. 337. are parallel to the crystallographic axes and

Fig. 338.

indicated thus:

!+!+!= 3 axes.

c) Center. This element of symmetry

is also present and demands parallelism

of faces. Figure 338 shows the above

elements of symmetry.

Orthorhombic bi pyramids. The form

whose faces possess the parametral ratio, a : b :

c, is known as the

unit or fundamental orthorhombic bipyramid. It consists of

eight similar scalene triangles, figure 339. The symbols according

to Naumann and Miller are as follows:

P, {nij.

Fig. 339. Fig. 340. Fig. 341.

The outer form, in figure 340, possesses the ratio a :

b

: me

(in > o < oc). In this case m = 2. This is a modified orthorhombic

bipyramid. Its symbols are :

mP, \hhl\.

In figure 341, the heavy, inner form is the unit bipyramid. The

lighter bipyramids intercept the b and c axes at unit distances but the

ORTHORHOMBIC BIPYRAMIDAL CLASS. 117

a axis at distances greater than unity. Their ratios may, however,

be indicated in general as,

na :

b :

me, (n > I ;

m

> o < 00 ).

These are the brachybipyramids, because the intercepts along the

br achydiagonal are greater than unity.' The Naumann and Miller

symbols are: mPn, \hkl\.

Fig. 342. Fig. 343.

Figure 342 shows two bipyramids (outer) which cut the a axis at

unity but intercept the b axis at the general distance nb, (n > i).

me. Since the

The ratios would, therefore, be expressed by a : nb :

intercepts along the macrodiagonal are greater than unity, these are

called macrobipyramids* The symbols according to Naumann and

Miller are mPn, \khl\.

Figure 343 shows the

relationship existing between

the unit, macro-, and

brachy bipyramids, while

figure 344 shows it for the

unit, modified, and macrobipyramids.

Prisms. Similarly

there are three types of

prisms, namely, the unit,

macro-, and brachyprisms . Fig. 344.

Each consists of four faces,

cutting the a and b axes, but extending parallel to the c axis

118 ORTHORHOMBIC SYSTEM.

Figure 345 represents

a tmit-prism with

the following symbols:

a \b :

act, ooP, {no}.

The brachyprism is

shown in figure 346. Its

symbols are:

is

na\b\ oo^,

\hko\

In figure 347, there

a unit prism surrounded

by a macroprism, whose symbols

may be written:

a : nb :

ccc, ocPn, \kho\.

For the

relationship existing

between these three prisms compare

figure 343.

Domes. These are horizontal

Fig. 347. prisms and, hence, cut the and

one of the horizontal axes. Domes,

which are parallel to the a axis or brachydiagonal, are called brachydomes.

Their general symbols are:

oca :

b :

me,

mP\$o, \ohl\, figure 348.

Those, which

extend parallel to

the

macrodiagonal,

are termed

macro domes,

figure 349. Their

symbols are:

\hol\.

.

Fig. 348. Fig. 349.

As is obvious,

prisms and domes

ORTHORHOMBIC BIPYRAMIDAL CLASS. 119

are open forms and, hence, can only occur in combination with other

forms.

Pinacoids. These cut one axis and

extend parallel to the other two. There

are three types, as follows:

Basal pinacoids, ooa: Oo5 :

c, OP,

{001 j.

Brachypinacoids,

120 ORTHORHOMBIC SYSTEM.

diagram :

Relationship of forms. This is to be seen from the following

ooPoo ooPn OOP oo Pn ocPoo

Fig. 351.

Fig. 352. Fig. 353.

Fig. 354.

Combinations. Figure 351. ^=ooP, {no}; e = P2, {122}.

Brookite, TiO 2

.

Figure 352. c = OP, {ooi}; * = iP, {113}; e = fPoc, Jo23}.

Chalcocite, Cu 2

S.

Figure 353. P = P, fin}; s = lP, ju 3 }; c = OP, \ooi\.

Sulphur, S.

Figure 354. m=ooP, }iio}.; b = ooPoo, }oio}; k = Poo,

ion}. Aragonite, CaCO 8

.

Figure 355. a = OoPoo, j 100} ;

5 = OoP2, 1 120} ;

b = OcPoo,

{oio}; o = P, jiii}; ^ = 2 P2, \2ii\-

t = PS) t \on}. Chrysoberyl,

Be(AlO 2 )2 .

ORTHORHOMBIC PYRAMIDAL CLASS. 121

Fig. 355.

Fig. 356. Fig. 357.

Fig. 358.

Figure 356. m = ooP, \ i

io\ ;

/ = ooP2,

JI20J; ^ = 2Pdo, {021}; o = P, jiuf. Topaz,

Al 2(F.OH) 2

Si0 4

.

Figures 357 to 359. m = OoP, S

I][

o!;

w = OoP|, J320jj

= ocPoc, j loof ;

z = P,

{in}; 17 == fPf, {324};

122 ORTHORHOMBIC SYSTEM.

ORTHORHOMBIC BISPHENOIDAL CLASS. 123

Combinations. Figure 361. a = ooPoo, |ioo}; g-

= ooP,

}noj; b =ooPo6, joio}; o =

3 Poo

;

r = -u, ou

;

124 ORTHORHOMIC SYSTEM.

gonal systems, respectively, in that faces lying wholly

octants are extended.

within alternate

Orthorhombic Msphenoids. Figure 365 shows the application

of the sphenoidal hemihedrism to an orthorhornbic bipyramid, which

yields two new correlated,

enantiomorphous forms, called the right,

figure 366, and left, figure 364, orthorhornbic bisphenoids. These

forms are bounded by four scalene triangles. The crystallographic

axes bisect the edges.

Fig. 364. Fig. 365. Fig.. 366.

Since there are several types of orthorhombic bipyramids,

it follows

that each will yield two enantiomorphous bisphenoids. They

are termed the orthorhombic bisphenoids. These are given and

their symbols indicated in the tabulation on page 125.

All other forms must occur with the full number of faces, that is,

they are apparently holohedral.

ORTHORHOMBIC BISPHENOIDAL CLASS. 125

Combination. Figure 367. m = ooP, {noj;

P - P

/

, { 1 1 1 } ;

z = r

, 1 1 1 1 } . Epsomite, MgSO4 +

2 2

Fig. 367.

MONOCLINIC SYSTEMS

Crystallographic Axes. To this system belong those forms

which can be referred to three unequal axes, two of which (a' and c)

intersect at an oblique angle, while the

p I*/

-a.

third axis (b) is

perpendicular to -these

two. The oblique angle between the a'

and c axes is termed ft. Figure 368

shows an axial cross of this system.

T It is customary to place the b axis so

as to extend from right to left. The

+tf axis is held vertically. The a' axis is then

directed toward the observer.

a' axis is inclined,

Since the

it is called the clinoaxis.

The b axis is often spoken of as

Fig 368. the ortho-axis. The obtuse angle between

the a' and c axis is the negative

angle ft, whereas the acute angle is positive. Obviously, they are

supplementary angles. The elements of crystallization consist of the

axial ratio and the angle ft, which may be either the obtuse or the

acute angle. Compare page

8.

Classes of Symmetry. The monoclinic system

classes of symmetry, as follows:

includes three

1. Prismatic class (Holohedrism^)

2. Domatic class (Hemihedrism.)

3. Sphenoidal class (Hemimorphism.)

The first class is

the most important.

/. MONOCLINIC PRISMATIC CLASS. 2 )

(Holohedrism.}

This class possesses one plane of symmetry, which

Symmetry.

includes the a' and axes and, hence,

is directed toward the observer.

system.

i) Also termed the clinorhombic, hemiprismatic, monoelinohedral, monosymmetric or oblique

3) Normalgroup of Dana. 

MONOCLINIC PRISMATIC CLASS. 127

Perpendicular to this plane, that is, parallel

to the b axis, is an axis of binary symmetry.

A center of symmetry is also present.

Figure 369 shows these elements in a crystal

of augite. These elements are represented

diagrammatically in figure 370, which is a

projection of a monoclinic form upon the

plane of the a' and b axes.

Hemi-pyramids. On account of the

presence in this class of only one plane of

symmetry and an axis of binary symmetry,

Fig. 369.

a form with unit intercepts, that is, with

the parametral ratio a' b : : c, can possess

but four faces. Figure 371 shows four

such faces, which enclose the positive angle

ft and are said to constitute the -positive

unit hemi-pyramid.^ Figure 372 shows

four faces with the same ratio enclosing the

Fig. 370.

Fig. 371. Fig. 372. Fig. 373.

negative angle /?, and comprising the negative unit hemi-pyramid.

It is obvious that the faces of these hemi-pyramids are dissimilar,

those over the negative angle being the larger. The symbols for these

hemi-pyramids are according to Naumann and Miller, -HP j iilj and

P 1

1 1 1 { , respectively. Two unit hemi-pyramids occurring simultaneously

constitute the monoclinic unit bipyramid, figure 373.

i) The term hemi-bipyramid ought more properly be employed because of the fact that we are

dealing with four faces of a bipyramid and not of a pyramid as the term has hitherto been used.

128 MONOCLINIC SYSTEM.

Since this system differs essentially from the orthorhombic in the

obliquity of the a axis, it follows that modified, clino, and ortho

hemi-pyramids are also possible. They possess the following general

symbols:

Modified hemi-pyramids,

_(a' : b : me), w>o

Clino hemi-pyramids,

(na' : b : me), n>\;

m?n' \hkl\\

hkl\, hi; + nt?7i [hk7\\ - -mV T i

\hkl\\ h>k.

was

oc oc h k o n i

Fig. 375. Since the a' axis is inclined to the

Prisms. As the case in the

orthorhombic system, page 1

17, there are

also three types of prisms possible in this

system, namely, unit, clino-, and orthoprisms.

These forms cut the and b

'

axes and extend parallel to the vertical

axis.

The general symbols are:

Unit prism,

a' : b :

ace, ooP, j iiof, figure 374.

Clinoprism,

na' : b :0cc, ooPn', \hko\\ n>i,

h

MONOCLINIC PRISMATIC CLASS. 129

parallel to the b axis consist of but two faces. Figure 376 shows

such faces enclosing the positive angle and are termed the positive

hemi-orthodomc, whereas in 377 the negative hemi-orthodome is

Fig.

376. Fig. 31 Fig. 378.

represented. It is evident that the faces of the positive form are

always the smaller. Figure 378 shows these hemidomes in combination.

Their general symbols are:

Positive hemi-orthodome,

a' : ccZ> :

me, + ;wPoc, \hol\.

Negative hem i-orth odome,

a' : GC& :

m, mPtt, \hol\.

Pinacoids, There are three types of pinacoids possible

monoclinic system, namely,

Basal pinacoids, oca' : ccb :

c,

in the

OP, jooi \.

ooPoo',

Clinopinacoids, oca' : b : 00 r,

joio}.

Orthopinacoids, a' : ccb :

occ,

OOPOC, \100\.

These are forms consisting of but

two faces. Figure 379 shows a combination

of these pinacoids.

All forms of the monoclinic system

are open forms and, hence, every crystal

of this system is a combination. Fig. 379.

A summary of the forms of this class is

given as follows:

130 MONOCLINIC SYSTEM.

MONOCLINIC PRISMATIC CLASS. 131

a

TTl

Fig. 381. Fig. 382. Fig. 383.

Combinations. Figure 380. m =ooP, jnof; b= ooPoo',

Joio}; p=P, jmf. Gypsum, CaSO 4

.2H 2

O.

Figure 381. c = OP, |ooj|; m ooP, jno|; =ooPoo',

{010} ; j = 2Pob, J20i{. Orthoclase, KAlSi 3

O 8

.

Figure 382. m=aoP, juof;

132 MONOCLINIC SYSTEM.

{201 J ;

q

---- Poc' f

jouS

;

TT == 2 P2, J2if}; I =

S 3 1 1 } I = P3, I 3 i 3 j ;

*

Pr 2 (S0 4)8

.8H 8

0.

= 3P3, i 3 1 1 ! Praseodymium sulphate,

2. MONOCLINIC DOMATIC CLASS. 1 )

( Hemihedrism. )

^

^

-*-_

Symmetry. This class possesses but one

element of symmetry, namelv, a plane of

symmetry as shown in figure 387.

Tetra-pyramids. Since the axis of

Fig" 387. binary symmetry is lost, it follows that the

hemi-pyramids now yield two tetra-pyramids.

These forms consist of but two faces which are situated symmetrically

to the plane of symmetry. For example, in figure 371 the positive

hemi-pyramid yields the lower positive tetra-pyramid which consists

of the two faces in front, and the upper positive , tetra-pyramid

made up of the other two faces. In like manner the negative

hemi-pyramid yields the upper and lower negative tetra-pyramids.

Their symbols are given in the tabulation on page 133.

Hemi-clinodomes. Obviously, the clinodome is now divided

into an upper and a lower hemi-clinodome.

Tetra-domes. The hemi-orthodomes yield upper and lower

tetra-domes.

Hemi-prisms. Each prism now yields two hemi-prisms, designated

as front and rear forms.

Pinacoids. The clinopinacoids must on account of the symmetry

occur with the full number of faces, namely, two. The basal

and orthopinacoids each yield two forms. In the case of the basal

pinacoid, they are designated as upper and lower forms, while the

terms front and rear are employed for the orthopinacoids.

follows :

The forms and their general symbols may

be tabulated as

*) Clinohedral group of Dana.

MONOCLINIC DOMATIC CLASS. 133

134 MONOCLINIC SYSTEM.

a =

OP

Combination. Fig. 388. c 21, {ooi};

ooPoo

/, jioo|, and OOPX) r, j

100 J ; ;;/ =

ocP

OOP -

. Pet'

/, {-no}, and r, JUO{; q

=

u,

{on}; v = + -y-

/,

Fig. 3.8.

Tetrathionate of potassium, K a

S 4

O e

.

MONOCLINIC SPHENOIDAL CLASS. 135

3. MONOCLINIC SPHENOIDAL CLASS. 1 )

( Hemimorphism. )

Symmetry. A polar axis of binary

symmetry is the only element of symmetry /

present, figure 389. The forms of this

class are hemimorphic along the b axis,

which is now a singular axis. XN

X /

Those forms which extend parallel to

Fig. 389.

b axis, the orthodomes, basal and orthcpinacoids,

are unaltered. The others yield right and left forms, for

example, the unit prism yields the right and left hemi-prisms.

The forms and their symbols are tabulated as follows:

SYMBOLS

Dan.i terms this class the hemimorphic group.

136 MONOCLINIC SYSTEM.

Combinations.

Figures 390 and 391.

a = OoPoo, |

c =

; looj;

OP, Jooij; r= -Poc,

OOP

!

ioi j; p

-- :

r

no = I

2

OCP

Fig. 390. Fig. 391. POO'

q ---- I - ,

MONOCLINIC SPHENOIDAL CLASS. 137

Poc'

{on} (figure 390); q = r

,

{on|

(figure 391). These combinations

occur on tartaric acid, C 4

H 6

O 6

. The

above figures represent

left- and right-handed crystals.

TRICLIN1C SYSTEM.

Crystallographic Axes. This system includes all forms which

can be referred to three unequal axes intersecting each other at

oblique angles. The axes are designated

+ c

as in the orthorhombic system, namely,

,

brachydiagonal; b, macrodiagonal; and

_j

^/O*'

-c

Fig. 3,)2.

c, vertical axis. From this it follows

that one axis must be held vertically, a

second is directed toward the observer,

and then the third is inclined from right

to left or vice versa. Usually the

brachydiagonal

is the shorter of the two

lateral axes. Figure 392 shows an axial

cross of the triclinic system. The oblique

angles between the axes are indicated as

follows: b /\ c = a, a A c = (3, and a A b

= y. The elements of crystallization

consist of the axial ratio and the *hree angles a, /?, and y, page 8.

Classes of Symmetry. There are but two classes of symmetry

in the triclinic system, namely:

1. Pinacoidal class (Holohedrism).

2. Asymmetric class (Hemihedrism).

The first is

the important class.

/.

Fig. 393. sist of but two faces, namely, face and parallel

PINACOIDAL CLASS. 2 )

Holohedrism.

( )

Symmetry. A center of symmetry

is the

only element present. Hence, forms can con-

counter-face. This is

represented diagrammat-

\

V 1-^

[O]

!) Also termed the anorthic, asymmetric or clinorhomboidal system.

2) Normal group of Dana.

PINACOIDAL CLASS. 139

ically by figure 393, which shows a triclinic combination projected

upon the plane of the a and 5 axes.

Tetra-pyramids. As already shown, triclinic forms consist of

but two faces. Therefore, since the planes of the crystallographic

axes divide space into four pairs of dissimilar octants, it follows that

four types of pyramidal forms must result. These are spoken of as

tetra-pyramids .^ There are, hence, four tetra-pyramids, each cutting

the axes at their unit lengths. The same is also true of the

modified, brachy- and macro- bipyramids. That is to say, the var-

-c

_

Fig. 394.

Fig. 395.

ious bipyramids of the orthorhombic system, on account of the obliquity

of the three axes, now yield four tetra-pyramids each. They are

designated as tipper right, upper left, lower rig-Jit, and lower left

forms, depending upon which of the front octants the form encloses.

Naumann indicates them in turn by P', 'P, P., ,P. The, general

symbols for all types are given in the tabulation on page 141.

394 shows the four unit tetra-pyramids in combination.

Figure

Henri-prisms. Obviously the prisms are now to be designated

as rig-ht and left forms. These two forms are in combination with

the basal pinacoid in figure 395.

In reality, tetra-bipyramids, see page 127.

140 TRICLINIC SYSTEM.

Hemi-domes. All domes now consist of but two faces. Hence,

we may speak of rig-Jit and left hemi-br achydomes, and upper and

lo^ver hemi-macrodomes . These

Fig. 396. Fig. 397.

forms are shown in combination

with the macro- and brachypinacoids, respectively, in figures 396 and

397-

Pinacoids. These forms occur with their usual number of faces

and are designated, as heretofore, by the terms basal, brachy-, and

I/

Fig. 398.

macropinacoids, depending upon the fact whether they extend parallel

to the c, a, or b axis. Figure 398 shows these pinacoids in

combination.

PINACOIDAL CLASS.

14 L

The various forms and symbols are given in the following table:

=

142 TKICLINIC SYSTEM.

Relationship of forms. The diagram on page 120 may be used

for this purpose, we if bear in mind that bipyramids, prisms, and

domes, indicated in the same, now represent four tetra-pyramids,

two hemi-prisms, and two hemi-domes, respectively.

Combinations. Figure 399. x

:

P'|ini; r = 'P \ni\\

Axinite, HCa 8

Al 2

BSi 4

O 16

.

Fig. 399. Fig. 400. Fig. 401.

Figures 400 and 401. m = ooP;|uoj; M = oo'PjuoJ;

b = ooPooioioS; c = OP{ooi}; x = ,P,oc{ io~i | ;

=

r == iP, 00)403 { - Albite, NaAlSi 3 8

.

P,{ui~};

2. ASYMMETRIC CLASS. 1 )

(Hemihedrism. )

Symmetry.

This class has no element of

symmetry. This is clearly shown by figure

402.

Forms, Since the center of symmetry is

lost, it follows that one face may constitute a

Fig. 402.

form and, hence, this class possesses ogdopyramtds,

tetra-prisms and tetra-domes , . The forms are designated

as in the preceding class, indicating, however, whether the

octant in which the form lies is in front or not. For example,

i )

Dana calls this the asymmetric group.

ASYMMETRIC CLASS. 143

- a :

I) : c, P'r, j

1 1 1 \ ,

is an ogdopyramid occupying

the upper right rear octant, while a : b :

-c, P,/~,

j i il is another

} ,

in the lower right front octant.

The various forms and their symbols are easily

deduced from those given on page 141.

Combinations. Figure 403. a ooPoc /,

jiooj; a' = ooPoo r, |ioo|; b = OcPdo r, joio(;

b' = ooPoo /, Jolo}; c = OP^, jooi|; c = OP/,

JooTj, ?^ = P'2r, jl22(;/ = P^/, \ioT\; strontium

bitartrate, Sr(C4H 4

O 6H) 2.4H 2

O.

COMPOUND CRYSTALS.

Fig. 404. Fig.

substances are observed grouped in this way.

Parallel Grouping. Oftentimes two crystals of the same substance

are observed to have so intergrown that the crystallographic

axes of the one individual

are parallel

to those of the other.

Such an arrangement

of crystals is

termed parallel

grouping. Figures

404 and 405^ show

such groups of quartz

and calcite,

respect-

405. ively. Occasionally,

crystals

of different

Twin Crystals. Two crystals may also intergrow so that, even

Fig. 406. Fig. 407.

though parallelism of the crystals is wanting, the growth has, nevertheless,

taken place in

some definite manner.

Such crystals are

spoken of as twin crystals,

or in short,

twins. Figure 406

illustrates such a twin

crystal commonly observed

on staurolite.

In twin crystals both

individuals have at least one crystal plane or a direction in common.

Figure 407 shows a twinned octahedron. The plane common to

both parts is termed the composition plane. In general, the

plane to which the twin crystal is symmetrical is the twinning

plane. In some instances, composition and twinning" planes

coincide. Both, however, are parallel to some possible face of the



After Tschermak and Melczer, respectively,

COMPOUND CRYSTALS. 145

crystal, which is not parallel to a plane of symmetry. The line or

direction perpendicular to the twinning plane is the twinning- axis.

A twinning la^v is

expressed by indicating the twinning plane or

axis.

Twin crystals are commonly divided into two classes: i) Contact

or Juxtaposition twins, and 2) Penetration twins. ^ These

are illustrated by figures 407 and 406, respectively. Contact twins

consist of two individuals so placed that if one be rotated through

1 80 about the twinning axis the simple crystal results. In penetration

twins two individuals have interpenetrated one another. If one

of the individuals be rotated through 180 about the twinning axis

both individuals will occupy the same position.

Contact and penetration twins are comparatively common in all

systems. In studying twins, it must be borne in mind, as pointed out

on page 3, that the two individuals may not be symmetrical owing

Re-entrant angles are commonly indicative of twinning.

Common twinning laws. Cubic System. The most common

to distortion.

law in the cubic system is that known as the spinel law, where the

twinning plane is parallel to a face of an octahedron, O{in}.

Figure 407 shows such a twin crystal of the mineral spinel, while

figure 408 shows a twinned octahedron of magnetite. A penetration

Fig. 408. Fig. 409. Fig. 410.

twin of fluorite is shown in figure 409. Here, two cubes interpenetrate

according to the above law. Figure 410 shows a penetration

twin of two tetrahedrons, observed on the diamond. The twinning

plane is a plane parallel to a face of a cube, OoOoo{ioo}, which in

i) Also designated as reflection and rotation twins, because they are symmetrical to a plane and

an axis, respectively.

V? ** A ** vV

OF THE

UNIVERSITY

CF

146 COMPOUND CRYSTALS.

the hextetrahedral class is no longer a plane of symmetry. The axes

are parallel in the two individuals and since the twinning tends to

give the twin the symmetry of the hexoctahedral class, such twinned

Fig. 411.

crystals are sometimes spoken of as supplementary twins.

Of the minerals crystallizing in the dyakisdodecahedral

class, pyrite furnishes excellent

twins. Figure 411 shows a penetration

twin of two pyritohedrons of this mineral.

Such twins are often known as crystals of

the iron cross. A plane parallel to a face of

the rhombic dodecahedron, OcO {nof

is the

,

twinning plane. Such a plane is parallel to

the secondary planes of symmetry which are

not present in this class.

Hexagonal System. Calcite and quartz are the only common

minerals belonging to this system which furnish good examples of

twinning.

These minerals belong to the ditrigonal scalenohedral and

trigonal trapezohedral classes,

respectively.

Fig. 412. Fig. 413. Fig. 414.

Upon calcite the basal pinacoid, ORjoooi J, is commonly a twinning

plane. Figure 412 illustrates this law. 1 *

A plane parallel to a

face of the negative rhombohedron, --^R{oii2}, may also be a

twinning plane as illustrated by figure 413. These are the most

common laws on calcite although crystals possessing a twinning plane

parallel to a face of the rhombohedron, 2RJO22IJ, are also to be

noted.

Compare with figure 187.

COMPOUND CRYSTALS. 147

The so-called Brazilian law is common on twins of quartz, figure

414. Here, a right and left crystal have interpenetrated so that the

twin is now symmetrical to a plane parallel to a face of the prism

of the second order, OoP2 {1120}, compare figures 253 and 254.

Figure 414, as is obvious, possesses a higher grade of symmetry than

its

component individuals, namely, that of the ditrigonal scalenohedral

class.

Tetragonal System.

Most

of the twin crystals of this

system are to be observed on

substances crystallizing in the

ditetragonal bipyramidal class.

In this class a plane parallel to

a face of

the unit bipyramid of

the second order, Poo jouj,

commonly acts as the twinning

Fig. 415. Fig. 416.

plane. Figures 415 and 416

show crystals of cassiterite and zircon, respectively, twinned according

to this law.

Orthorhombie System. The most common twins of this system

belong to the bipyramidal (holohedral) class in which any face aside

from the pinacoids may act

as twinning plane. Figure

406, page 144, shows a penetration

twin of staurolite,

where the brachydome, -fPoc

{032}, acts as the twinning

plane. Figure 417 shows

the same mineral with the

pyramid, -fPf 5232;,

as the

twinning plane. Figure 418

represents a contact twin of aragonite. Here the unit prism, OoP

1 1 10}, is the twinning plane.

Fig. 417. Fig. 418.

Monoclinic System. In this system, gypsum and orthoclase

furnish some of the best examples. Figure 419 shows a contact

twin of gypsum in which the orthopinacoid, ooPoojioo},

is the

twinning plane. A penetration twin of orthoclase is shown in figure

148 COMPOUND CRYSTALS.

Fig. 419. Fig. 420. figure 421, the clinopinacoid, OoPoo |oioj,

420. Here, the orthopinacoid also acts as

twinning plane. This is known as the

Triclinic System. Since there are no

planes of symmetry in this system, any

plane may act as the twinning plane. The

mineral albite furnishes good examples. In

acts as the twinning plane. This is the

albite lazv. Another

common law is shown

by figure 422. Here,

the basal pinacoids

of both individuals

Fig. 421.

are parallel, thecrystallographic

b axis

acting as the twinning axis. This is known as the

fiericline law.

Repeated twinning. In the foregoing, crystals consisting of but

two individuals have been discussed. Intergrowths of three, four,

five,

etc., individuals are termed threelings, fourlings, fivelings, and so

Fig. 423. Fig. 424. Fig. 425.

on. Polysynthetic and cyclic twins are the result of repeated twinning.

In the polysynthetic twins the twinning planes between any two

individuals are parallel. This is illustrated by figures 423 and 424

showing polysynthetic twins of albite and aragonite, respectively. 1J

If the individuals are very thin the re-entrant angles are usually

1

) Compare with figures 418 and 421.

COMPOUND CRYSTALS. 149

indicated by striations. The cyclic twins result when the twinning

planes do not remain parallel, as for example when adjacent faces of

a form act as twinning planes. This is shown by the cyclic twins of

rutile, figure 425, in which adjoining faces of the unit bipyramid of

the second order OoP2 joi

i \

act as twinning planes.

Mimicry. As a

result of repeated twinning,

forms of an apparently

symmetry usually result.

This is especially

common with those

substances

possessing

pseudosymmetry, page Fig. 426.

94. Figure 426 shows

a trilling of the orthorhombic mineral aragonite, CaCO 3

which is

,

now apparently hexagonal in its outline. In figure 427 the crosssection

is shown. This phenomenon is called mimicry.

-t >'

oi"7

TABULAR CLASSIFICATION

SHOWING THB ELEMENTS OF SYMMETRY

AND THE SIMPLE FORMS

OF THB THtRTY-TWO CLASSES OF CRYSTALS.

CUBIC SYSTEM.

Classes of Crystals, I to 5.

(Page 150.)

TABULAR CLASSIFICATION SHOWING THE ELEMENTS OF SYMMETRY A*

/. CUBIC

1) The blank spaces indicate that the forms are apparently holohedral.

[1501



HEXAGONAL SYSTEM.

Classes of Crystals, 6 to II.

(Page 151.)

151 2. HEXAQO

HEXAGONAL SYSTEM.

(Continued)

Classes of Crystals, 12 to 17.

(Page 152.)

152 2. HEXAGC

(Co,

CLASS

12. Ditrigonal

Pyramidal

Trigonal Hemihedrisnt

wifli

Hemimorphism

1V"T

13. Hexagonal

Pyramidal

f Pyramidal Heini- 1

// c drism with i

A-

[^ Hemimorph

14. Trigonal

Bi pyramidal

r

Trigonal

"I

L Tetartohedrism }

1 5. Trigonal

Trapezohedral

r Trabezohedral 1

r 7 \Jfcta

1 6. Trigonal

Khombohedral

f Rhombohedral \

L, jfTetartohedrism j

17. Trigonal

Pyramidal

( Ogdohedrism )

TETRAGONAL SYSTEM.

Classes of Crystals, 18 to 24.

(Page 153.)

153 3. TETRA

MAL SYSTEM. 153

ORTHORHOMBIC SYSTEM.

Classes of Crystals, 25 to 27.

(Page 154.)

154 4. ORTHOR

WIC SYSTEM. 154

MONOCLINIC SYSTEM.

Classes of Crystals, 28 to 30.

(Page 155.)

155 5. MONOC

'1C SYSTEM. 155

TRICUNIC SYSTEM.

Classes of Crystals, 31 and 32.

(Page 1 56.)

156 6. TRIG*

7 SYSTEM. 156

INDEX.

Acid, tartaric, 137, 155

Albite, 8, 142, 148, 156

Albite Law, 148

Alum, 2

Amorphous structure, 1

substances, 2

Analcite, 24

Anatase, 99

Anglesite, 8

Angular position of faces, 14

Anorthic system, 138

Apatite, 68, 151

Apparently holohedral forms, 29

Aragonite, 8, 120, 147, 148, 149

Argentite, 24, 25

Asymmetric class, 142, 156

group, 142

system, 138

Axes, crystallographic, 4, 17, 43, 92, 115,

126, 138

of symmetry, 13

Axial cross, 4

Axial ratio, 7

Axinite, 142

Axis, polar, 16

singular, 16

Barite, 154

Barium nitrate, 42

Barium stibiotartrate and potassium

nitrate, 70, 151

Beryl, 53, 151

Bisphenoids, orthorhombic, 124

tetragonal, first order, 102, 111

second order, 111

Boracite, 32

third order, 113

Brachy bipyramids, 117

diagonal, 115, 138

domes, 118

prisms, -117

Brazilian law, 147

Brookite, 120

Calamine, 123, 154

Calcite, 64, 65, 144, 146, 151

Cassiterite, 99, 147, 153

Celestite, 121

Center of symmetry, 14

Chalcocite, 120

Chalcopyrite, 105, 153

Chemical crystallography, 2

Chrysoberyl, 120

Cinnabar, 85

Classes of crystals, 14, 150

Classification of the thirty-two classes

of crystals, 150

Clino-axis, 126

domes, 128

hemi-pyramid, 128

prism, 128

rhombic system, 126

rhomboidal system, 138

Clinohedral group, 132

Closed forms, 6

Cobaltite, 36

Coefficients, rationality of, 9

Combinations, 7

cubic, 23, 31, 35, 38, 42

hexagonal, 52, 55, 64, 68, 74, 76, 85,

89, 91

tetragonal, 98, 101, 104, 108, 111

orthorhombic, 120, 123, 125

monoclinic, 131, 134, 136

triclinic, 142, 143

Common twinning laws, 145

Composition plane, 144

Compound crystals, 144

Congruent forms, 16

Constancy of interfa^ial angles, 2

Contact twins, 145

Copper, 24

Correlated forms, 15

Corundum, 64, 65

Crystal faces, 2

forms, 6

habit, 4



158 INDEX.

Crystal system, 14

systems, 5

Crystalline structure, 1

Crystallization, elements of, 8

Crystallized substances, 2

Crystallographic axes, 4

cubic, 17

hexagonal, 43

tetragonal, 92

orthorhombic, 115

monoclinic, 126

triclinic, 138

Crystallography, 2

Crystals, 1, 2,

distorted, 3

formation of, 1, 2

Cube, 19

Cubic system, 5, 17, 150

Cyclic twins, 148

Dana's symbols, 11

Deltoid, 27

Diamond, 145

Didodecahedron, 34

Dihexagonal bipyramid, 48

bipyramidal class, 44, 151

prism, 50

pyramidal class, 53, 151

pyramids, 54

Diopside, 131

Dioptase, 89, 152

Diploid, 34

Distortion, 3

Ditetragonal bipyramid, 95

bipyramidal class, 93, 153

prism, 96

pyramidal class, 99, 153

Ditrigonal bipyramidal class, 56, 151

bipyramids, 57

prisms, 59, 72

pyramids, 71

pyramidal class, 70, 152

pyramidal tetartohedrism, 70

scalenohedral class, 60, 151

Dodecahedron, 19

deltoid, 27

pentagonal, 33

rhombic, 19

tetrahedral pentagonal, 39

Dolomite, 89

Domatic class, 132, 155

Dyakisdodecahedral class, 32, 150

Dyakisdodecahedron, 34

Elements of crystallization, 8

symmetry, 12

Epsomite, 125, 154

Etch-figures, 29

Faces, angular position of, 14

Fivelings, 148

Fluorite, 24, 145

Form, crystal, 6

Formation of crystals, 1, 2

Forms, congruent, 16

closed, 6

correlated, 15

Enantiomorphous, 16

fundamental, 6

hemi-morphic, 16

open, 6

unit, 7

Fourlings, 148

Fundamental forms, 6

Galena, 24, 150

Garnet, 25

Geometrical crystallography, 2

Gypsum, 8, 131, 147, 155

Gyroidal hemihedrism, 36

Gyroids, 37

Habit, crystal, 4

prismatic, 4

tabular, 4

Halite, 24, 29

Hematite, 64, 65

Hemi-bipyramid, 127

clinodomes, 132

domes, 140

Hemihedrism, 15

cubic, 26, 32, 36

hexagonal, 55

tetragonal, 101

orthorhombic, 123

monoclinic, 132

triclinic, 142

INDEX. 159

Hemimorphic forms, 16

group, hexagonal, 53

monoclinic, 135

orthorhombic, 121

tetragonal, 99

Hemimorphism, 16

hexagonal, 53, 70, 74, 89

monoclinic, 132

orthorhombic, 121

tetragonal, 99, 110

Hemimorphite >

103

Hemi-orthodomes, 129

Hemiprisms, monoclinic, 132

triclinic, 139

Hemiprismatic system, 126

Hemipyramids, 127

Hexagonal basal pinacoid, 51

bipyramidal class, 65, 151

bipyramid, first order, 45

second order, 46

third order, 65

hemihedrisms, 55

prism, first order, 50

second order, 50, 72

third order, 67, 87

pyramid, first order, 54

second order, 54, 71

third order, 75

pyramidal class, 74, 152

system, 5, 43, 151, 152

tetartohedrisms, 76

trapezohedral class, 68, 151

trapezohedrons, 68

Hexahedron, 19

Hexoctahedral class, 17, 150

Hexoctahedron, 21

Hextetrahedral class, 26, 150

Hextetrahedron, 28

Holohedral, apparently, 29

Holohedrism, 15

Icositetrahedron, 20

Incline-face hemihedrism, 27

Indices, Miller's, 12

lodyrite, 55

Iron cross, 146

Isometric system, 17

Juxtaposition twins, 145

Leucitohedron, 20

Limiting forms, 23

Macrobipyramids, 117

diagonal, 115, 138

domes, 118

prisms, 117

Magnetite, 25, 145

Miller's indices, 12

system, 12

Mimicry, 149

Modified hemi-pyramid, 128

pyramid, 7

Monoclinic domatic class, 132, 155

domes, 128

prismatic class, 126, 155

prisms, 128

sphenoidal class, 135, 155

system, 5, 126, 155

Monoclinohedral system, 126

Monosymmetric system, 126

Naumann symbols, 11, 62

Nepheline, 76

Nickel sulphate, 109, 153

Normal group, cubic, 17

hexagonal, 44

monoclinic, 126

orthorhombic, 115

tetragonal, 93

triclinic, 138

Oblique system, 126

Octahedron, 19

Octants, 17

Ogdohedrism, 15, 89

Ogdo-pyramids, 142

Open forms, 6

Ortho-axis, 126

Orthoclase, 131, 147, 148

Orthohemi-pyramid, 128

Ortho-prism, 128

Orthorhombic bipyramidal class, 115, 154

bipyramids, 116

bisphenoidal class, 123, 154

bisphenoids, 124

domes, 118

160 INDEX.

Orthorhombic pinacoids, 119

prisms, 117

pyramidal class, 121, 154

system, 5, 115, 154

Parallel-face hemihedrism, 32

grouping, 144

Parameters, 5

Parametral ratio, 5

Penetration twins, 145

Penta-erythrite, 101

Pentagonal dodecahedron, 33

hemihedrism, 32

icositetrahedron, 37

icositetahedral class, 36, 150

Pericline law, 148

Physical crystallography, 2

Pinacoidal class, 138, 156

Plagiohedral group, 36

hemihedrism, 36

Planes of symmetry, 12

Polar axes, 16

Pole, 53

Polysynthetic twins, 148

Potassium tetrathionate, 134, 155

Praseodymium sulphate, 132

Prismatic habit, 4

system, 115

Pseudosymmetry, 94, 149

Pyramid cube, 21

Pyramidal group, hexagonal, 65

tetragonal, 105

hemihedrism, hexagonal, 55, 65

system, 92

tetragonal, 101, 105

Pyrite, 30, 33, 35, 36, 146, 150

Pyritohedral group, 32

hemihedrism, 32

Pyritohedron, 33

Quartz, 8, 85, 144, 146, 147, 152

Ratio, axial, 7

parametral, 5

Rationality of coefficients, 9

Re-entrant angles, 148

Reflection twins, 145

Regular system, 17

Repeated twinning, 148

Rhombic dodecahedron, 19

Rhombic system, 115

Rhombohedral group, 60

hemimorphic, 70

hemihedrism, 55, 60

hemimorphic class, 70

tetartohedrism, 76, 85

Rhombohedron of the middle edges, 62

like forms, 71

Rhombohedrons, first order, 60, 81, 85

second order, 86

third order, 86

Rotation twins, 145

Rutile, 149

Salammoniac, 38, 150

Scalenohedron like forms, 71

Scalenohedrons, hexagonal, 61

tetragonal, 103

Scheelite, 108, 153

Siderite, 64

Silver fluoride, 101, 153

Singular axis, 16

Sodium chlorate, 42, 150

periodate, 91, 152

Sphalerite, 30, 31, 32

Sphenoidal group, orthorhombic, 123

tetragonal, 102

hemihedrism, 101, 102

Spinel, 24, 25, 145

law, 145

Staurolite, 144, 147

Steno, Nicolas, 4

Striations, 31, 149

Strontium antimonyl-tartarte, 76, 152

bitartrate, 143, 156

Structure, amorphous, 1

crystalline, 1

Struvite, 123

Strychnine sulphate, 109

Sulphur, 7, 120

Supplementary twins, 146

Sylvite, 29

Symbols, 10

Weiss, 11

Symmetry, axes of, 13, 14

INDEX. 161

Symmetry, center, 14

classes of, 14

elements of, 12

planes of, 12

Tabular habit, 4

Tartaric acid, 137, 155

Tesseral system, 17

Tessular system, 17

Tetartohedral group, cubic, 38

tetragonal, 111

Tetartohedrism, 15

cubic, 38

hexagonal, 76

tetragonal, 111

Tetra-bipyramids, 139

domes, monoclinic, 132

triclinic, 142

pyramids, monoclinic, 132

triclinic, 139

Tetrathionate of potassium, 134, 155

Tetragonal basal pinacoid, 97

bipyramidal class, 105, 153

bipyramids, first order, 93

second order, 94

third order, 105

bisphenoidal class, 111, 153

bisphenoids, first order, 102, 111

second order, 111

third order, 113

hemihedrisms, 101

prisms, first order, 96

second order, 96

third order, 105

pyramidal class, 110, 153

pyramids, first order, 110

second order, 110

third order, 110

scalenohedral class, 102, 153

scalenohedrons, 103

system, 5, 92, 153

trapezohedral class, 108, 153

trapezohedrons, 108

trisoctahedron, 20

tristetrahedron, 28

Tetrahedral group, 26

hemihedrism, 26

pentagonal dodecahedral class, 38, 150

dodecahedron, 39

Tetrahedrite, 31, 150

Tetrahedron, 26

Tetrahexahedron, 21

Thirty-two classes of crystals, 14, 150

symmetry, 14, 150

Thorium sulphate, 131

Threelings, 148

Topaz, 8, 121

Tourmaline, 74, 152

Trapezohedral group, hexagonal, 68

tetragonal, 108

trigonal, 81

hemihedrism, hexagonal, 56, 68

tetragonal, 101, 108

tetartohedrism, 76

Trapezohedron, 20

Trapezohedrons, hexagonal, 68

tetragonal, 101, 108

Triclinic system, 5, 138, 156

Trigonal bipyramidal class, 76, 152

bipyramids, first order, 56, 77

second order, 77, 81

third order, 78

hemihedrism, 55, 56

prisms, first order, 56, 72, 77

second order, 77, 83

third order, 78

pyramids, first order, 70, 90

second order, 90

third order, 90

pyramidal class, 89, 152

rhombohedral class, 85

tetartohedrism, 76

trapezohedral class, 81, 152

trapezohedrons, 81

trisoctahedron, 20

tristetrahedron, 28

Trillings, 148, 149

Trimetric system, 115

Trisoctahedron, 20

tetragonal, 20

trigonal, 20

Tri-rhombohedral group, 85

Tristetrahedron, tetragonal, 27

trigonal, 28

Twin crystals, 144

162 INDEX.

Twinning axis, 145

law, 145

plane, 144

Twins, 144

contact, 145

juxtaposition, 145

penetration, 145

reflection. 145

rotation, 145

Unit form, 7

Urea, 104

Weiss, Prof. C. S., 11

symbols, 11

Wulfenite, 111, 153

Zincite, 55, 151

Zircon, 8, 98, 147

UNIVERSITY OF CALIFORNIA LIBRARY

This book is DUE on the last date stamped below.

Fij

NOV 10 1947

LIBRARY USE

JUL 2 1959

REG'D LD

MAR161959B JUL

LIEHASY 'J

AUG

AUG

REC'D

AUG

LD

LD

16Ju!'5SHj

JUN

81953LU

JUL 16

JAN 171954 LU

LD 21-100m-12,'46(A2012si6)4120

V.

..

UNIVERSITY OF CALIFORNIA LIBRARY

More magazines by this user
Similar magazines